Journal of Power Sources 449 (2020) 227596
Contents lists available at ScienceDirect
Journal of Power Sources journal homepage: www.elsevier.com/locate/jpowsour
Cathode materials for rechargeable zinc-ion batteries: From synthesis to mechanism and applications Changgang Li a, Xudong Zhang a, **, Wen He a, *, Guogang Xu b, Rong Sun a a b
College of Material Science and Engineering, Qilu University of Technology (Shandong Academy of Sciences), Jinan, 250353, China College of Material Science and Engineering, Shandong University of Science and Technology, Qingdao, 266590, China
H I G H L I G H T S
G R A P H I C A L A B S T R A C T
� Various cathode materials of zinc-ion batteries are reviewed and summarized. � Synthesis, composition, electrochemical properties and reaction mechanisms are highlighted. � Influences of electrolyte and anode on the performances are also analyzed. � Strategies, recommendations and di rections on future research are provided.
A R T I C L E I N F O
A B S T R A C T
Keywords: Zinc-ion battery Cathode material Synthesis Mechanism Electrolyte
Rechargeable zinc-ion batteries (RZIBs) are one of the most promising candidates to replace lithium-ion batteries and fulfill future electrical energy storage demands due to the characters of high environmental abundance, low cost and high capacities (820 mAh g 1/5855 mAh cm 3). Although some progresses have been made in enhancing the electrochemical performance of RZIBs, challenges of the lack of suitable cathodes to tolerate the stable insertion/extraction of Zn2þ ions still remain. In this review, we mainly summarize the synthesis tech nology, composition, structure and electrochemical properties of various cathode materials of RZIBs as well as optimization of the electrolyte, which include manganese-based oxides, vanadium-based materials, Prussian blue analogues, Chevrel phases, polyanionic compounds, metal disulfides, organic compounds, aqueous electrolyte and nonaqueous electrolyte. Furthermore, their energy storage mechanisms are also discussed. Finally, chal lenges, further research directions and perspectives regarding the development of high performance cathodes are highlighted. This review will be beneficial for researchers to develop high performance RZIBs for meeting the demands of rapidly developing electric vehicles and portable electronic products.
1. Introduction The development of rechargeable batteries plays a vital role in the
energy storage industry. In the past few decades, lithium-ion batteries are widely used for mobile electronics and electric vehicles due to the high energy density and mature markets [1–7]. However, lithium-ion
* Corresponding author. ** Corresponding author. E-mail addresses: [email protected]
(X. Zhang), [email protected]
(W. He). https://doi.org/10.1016/j.jpowsour.2019.227596 Received 17 August 2019; Received in revised form 6 December 2019; Accepted 8 December 2019 Available online 12 December 2019 0378-7753/© 2019 Elsevier B.V. All rights reserved.
C. Li et al.
Journal of Power Sources 449 (2020) 227596
cycling behavior and flexible negative electrode by electrodepositing Zn on carbon fibers, which offers an efficient solution to inhibit the growth of dendritic zinc. Parker et al.  used 3D Zn sponges to elevate the performance of the alkaline Zn//Ni(OH)2 battery, achieving an incredible long cycle life without Zn dendritic formation after ~54000 cycles. Kang et al.  prepared a Zn composite anode by mixing zinc particles with activated carbon to improve the cycle performance of RZIBs. Li et al.  fabricated a RZIB based on a new intercalated Na3V2(PO4)2F3 cathode coupled with carbon film functionalizing Zn anode and 2 M Zn(CF3SO3)2 electrolyte. The carbon film functionalizing Zn anode was prepared by rolling 80 wt% carbon black (super P) and 20 wt% polytetrafluoroethylene (PTFE) into thin carbon film (thickness, ~0.1 mm) and then placed it on the surface of a Zn foil. These methods mentioned above largely circumvent the plague of dendritic growth. As for the problem of hydrogen evolution in aqueous electrolytes, explo ration of organic electrolytes  and ionic liquid electrolytes  has been reported in RZIBs. However, most of the ionic liquid have imida zolium and pyrrolidinium cations, trifluoromethylsulfonate (TfO–), bis (trifluoromethylsulfonyl)amide (TFSA–) and dicyanamide (DCA–) counter ions, causing their application to be limited by eco-toxicity, biodegradability and biocompatibility . Bio-ionic liquid (choline)- water mixture might be a promising electrolyte for RZIBs because it is nontoxic, cheap and bio-degradable. The biggest challenge blocking application of RZIBs is the lack of cathode materials with high reversible capacity, excellent cycle stability and adequate operating voltage. Divalent Zn2þ ions show strong elec trostatic interactions with the host structures and large steric hindrance effects, inducing the poor cyclability and extremely slow intercalation kinetics [34,35]. It is apparent that the design rules for multivalent ions storage/intercalation processes are fundamentally different than that of monovalent ions. Many materials are currently reported as cathode for RZIBs, including manganese-based oxide, vanadium-based materials, Prussian blue analogues, Chevrel phases, polyanionic compounds, metal disulfides and organic compounds. As seen from Table 2, the number of annual publications on various reviews of RZIBs continues to increase rapidly in the past two years. These reviews mainly focus on the energy storage mechanism, electro chemical activation and challenges of RZIBs as well as recent develop ment of electrode materials. Though few important reviews have summarized the recent advances and prospects of RZIBs from different aspects (Table 2) [13–16,25,31,170], we shall present a different review in order to help readers readily understand the important roles of reasonable design and synthesis technology of cathode materials in improving the electrochemical performances of RZIBs. In this review, we mainly focus on the design and synthesis technology of various cathode materials for RZIBs in aqueous and nonaqueous electrolyte. The syn thetic methods, composition, structure, morphologies, electrochemical properties and reaction mechanisms of various cathode materials are
Table 1 Comparison of the characteristics of zinc metal with those of other metals [13, 14,19,21]. Category
Cation radius (Å) Atomic weight (g mol 1) Density (g cm 3) Volumetric capacity (mAh m 3) Gravimetric capacity (mAh g 1) Cost (USD kg 1) Abundance rank E (vs. the SHE) (V)
2.2 25 0.76
19.2 33 3.04
3.1 6 2.71
2.2 8 2.37
13.1 7 2.93
1.9 3 1.76
batteries suffer from complicated issues, such as safety, lack of lithium resources and environmental concerns, which led to the extensive exploration of new battery chemistries. Sodium-ion batteries have been considered as promising alternative to lithium-ion batteries for energy storage applications because of the abundant sodium reserves [8–12]. But it is difficult to find host materials with open structure for reversible Naþ insertion/deintercalate since the larger size and sluggish diffusion kinetics of Naþ as compared to Liþ. Developing renewable energy and expanding electric transportation require high energy density, fast charge/discharge time and environmentally friendly battery technol ogy. Therefore, researchers turn their attention to rechargeable multivalent-ion batteries, such as rechargeable zinc-ion batteries (RZIBs) [13–16], magnesium-ion batteries [17,18], calcium-ion batte ries [19,20] and aluminum-ion batteries [21,22]. Among them, RZIBs have particularly advantages in the following aspects (Table 1). Firstly, zinc metal is naturally abundant, inexpensive (USD $2 kg 1), and nontoxic . Secondly, as an anode it offers high gravimetric (820 mAh g 1) and volumetric capacities (5855 mAh cm 3). Moreover, zinc metal can also be used in both organic and aqueous electrolytes. It possesses not only a low redox potential ( 0.76 V vs. standard hydrogen electrode) compared to other metal anodes in aqueous electrolytes, but also two-electron transfer mechanism during cycling responsible for the high energy density. However, the application of RZIBs in practical energy storage devices still face substantial challenges because of the formation of Zn dendritic structures and the passivation layer on Zn electrode during charging, which hinders Zn2þ diffusion, resulting in capacity fade, short cycle life, and safety issues [24,25]. In addition, the standard electrode potential of Zn2þ ion deposition in aqueous electrolytes is more negative than that for hydrogen evolution, and this could pose a challenge to electrolyte stability in the aqueous phase . In order to restrain the Zn dendrite, coating and morphological optimization for Zn electrode have proven to be very effective strategies. Wang et al.  achieved dendrite-free Table 2 Comparison of various reviews of RZIBs. Published journal
Adv. Funct. Mater. J. Mater. Chem. A
28 (2018) 1802564 7 (2019)1820918236 135 (2019)58–84 3 (2019)1800111
Recent Advances in Zn-Ion Batteries
Crystal structures of cathode materials and Zn ion storage mechanisms Recent developments and challenges of cathode materials Reaction mechanism of cathode materials Mechanisms of electrochemical activation, insertion, and conversion occur Comprehensive overview and summary of cathode materials Energy storage mechanisms and types and challenges of cathode materials Challenges and recent developments of Zinc-Ion Batteries Synthesis technology, composition and optimization of cathode materials
Mater. Sci. Eng., R Adv. Sustainable Syst. Adv. Mater. Interfaces ACS Energy Lett. ACS Energy Lett. Our review
6 (2019)1900387 3 (2018)24802501 3 (2018) 2620 2640
A review on recent developments and challenges of cathode materials for rechargeable aqueous Zn-ion batteries Zinc-ion batteries: Materials, mechanisms, and applications Progress in Rechargeable Aqueous Zinc- and Aluminum-Ion Battery Electrodes: Challenges and Outlook Recent Advances and Prospects of Cathode Materials for Rechargeable Aqueous Zinc-Ion Batteries Recent Advances in Aqueous Zinc-ion Batteries Present and Future Perspective on Electrode Materials for Rechargeable Zinc-Ion Batteries Cathode materials for rechargeable zinc-ion batteries: from synthesis to mechanism and applications
     
C. Li et al.
Journal of Power Sources 449 (2020) 227596
hexagonally close-packed (hcp) oxide ions to form basic MnO6 octahe dral units, and these units are linked by edges and/or corners. The different linkages between the fundamental MnO6 octahedral units can form various polymorph crystallographic structures . Many poly morphic MnO2, such as α-MnO2, β-MnO2, γ-MnO2, ε-MnO2, δ-MnO2 and todorokite-type MnO2 have been used in cathode materials of RZIBs up to now. Table 3 is tunnel feature and tunnel size of different MnO2 forms.
Table 3 Tunnel type and size of different crystallographic forms of MnO2 . MnO2 form
(1 � 1), (2 � 2) (1 � 1) (1 � 1), (1 � 2) interlayer distance (3 � 3)
1.89, 4.6 1.89 1.89, 2.3 7.0 7.0
β-MnO2 γ-MnO2 δ-MnO2 Todorokite MnO2
2.1.1. α-MnO2 Xu et al.  prepared α-MnO2 cathode via a simple self-reacting microemulsion method using KMnO4 as raw material, iso-octane as solvent and surfactant sodium bis (2-ethylhexyl) sulfosuccinate as reductant. They first proposed a charge storage mechanism established on the migration of Zn2þ ions between this cathode and zinc anode in mild ZnSO4 or Zn(NO3)2 aqueous electrolyte (Fig. 1a). This RZIB pro vides a high capacity of 210 mAh g 1 at 0.5 C, which is higher than the capacity of alkaline Zn/MnO2 battery (125 mAh g 1) . The discharge capacity is about 100 mAh g 1 at 6C, and the Coulombic ef ficiency is about 100% after 100 cycles, indicating a high utility of electric capability. The cyclic voltammograms (CV) in Fig. 1b confirmed that the two distinguishable peaks at around 1.3 and 1.7 V are Zn2þ ions storage/release into/out of crystalline α-MnO2 tunnels to form ZnMn2O4. After that, the group of Xu  continued to investigate the storage process of Zn2þ insertion into α-MnO2 by electrochemical impedance spectrum. The results show that the storage process of alkaline (Liþ, Naþ, or Kþ) or alkaline-earth (Mg2þ, Ca2þ, or Ba2þ) metal cations in α-MnO2 can be divided into four steps: (1) transfer of hydrated cations from the electrolyte to the surface of the MnO2 electrode; (2) hydrated cations migration to the surface MnO2 particles from the
comprehensively discussed. Reaction mechanisms, including Zn2þ insertion/extraction, chemical conversion, Hþ/Zn2þ co-insertion/extraction, displacement and cation and anion co-intercalation mechanism are systematically analyzed. Moreover, the merits and key issues as well as the optimization strategies related to various cathodes and electrolytes are discussed. Finally, the recently explored cathodes, flexible zinc-ion battery, challenges, recent research trends and directions on cathode materials that can improve the battery performance are also presented. This review hopes to reveal particular strategies which may facilitate future developments of RZIBs. 2. Manganese-based oxide 2.1. MnO2 Manganese dioxide (MnO2) has been widely used as cathode mate rials of various batteries, such as zinc-manganese batteries, lithium-ion batteries and supercapacitors, because it is electrochemically active, environmentally friendly, and relatively cheap [36–40]. In MnO2 poly morphic crystal structure Mn4þ ions occupy octahedral pores formed by
Fig. 1. (a) Schematic diagram of the aqueous RZIB, the inset shows MnO6 octahedron structure in MnO2. (b) Cyclic voltammograms of the zinc anode (red line) and the α-MnO2 cathode (blue line) at 2 mV s 1 in 0.1 mol L 1 Zn(NO3)2 electrolyte. Reproduced with permission from Ref. , Copyright 2012 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim. (c) Schematic diagrams illustrating the mechanism of zinc intercalation into α-MnO2. Green octahedra and white, red, and turquoise spheres represent MnO6, Kþ, H2O, and Zn2þ, respectively. Reproduced with permission from Ref. , Copyright 2014 Springer Nature Limited. (For interpretation of the references to color in this figure legend, the reader is referred to the Web version of this article.) 3
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Fig. 2. (a) The charge-discharge profiles of the zinc/α-MnO2 for the first two cycles at a scan rate of C/20 (1C ¼ 210 mA g 1 of the active mass). (b) The corre sponding in situ XRD patterns during the electrochemical cycling. The regions of interest are described as I, II, III, and IV in (a). Reproduced with permission from Ref. . Copyright 2015 The Royal Society of Chemistry. (c) Crystal structure of Zn4(OH)6SO4⋅5H2O. Reproduced with permission from Ref. . Copyright 2016 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim.
porous MnO2 electrode; (3) dehydration of hydrated cations at solid/ electrolyte interface; and (4) diffusion of cations in the MnO2 lattice [45–47]. This storage process of Zn2þ ions is mainly determined by the phase change while there are no significant phase changes when MnO2 stores alkaline or alkaline-earth metal cations. With the decrease of potential, Zn2þ ions insert into MnO2 and form a new ZnMn2O4 phase, which leads to the increase of phase change resistance. Lee et al.  also synthesized a crystalline α-MnO2 nano-rod cathode by hydrothermal method using KMnO4 as raw material at 140 � C for 24 h. They investigated the intercalation mechanism of Zn2þ ions into α-MnO2 cathode during discharge/charge reactions, which undergoes a reversible phase transition of MnO2 from tunneled to layered polymorphs. The manganese decomposed from α-MnO2 during discharge process formed layered Zn-birnessite. The structure of Zn-birnessite is most likely an analogue of chalcophanite ((Zn, Mn) Mn3O7⋅3H2O) with P-1 space group, and the interlayer distance of layered Zn-birnessite is approximately 7 Å [49,50]. The substantial manganese decomposed from the cathode was dissolved into the elec trolyte (1.0 M ZnSO4 solution) during discharge process. In discharging process, almost 1/3 manganese in the α-MnO2 electrode is dissolved to form Zn-birnessite. However, the Mn concentration in electrolyte become negligibly small during charging, which means that dissolved Mn2þ ions completely recovered to combine with Mn vacancy sites of the layered structure to form the original α-MnO2. The mechanism of zinc intercalation into α-MnO2 is shown in Fig. 1c. About a year later, Lee et al.  also elucidated the intercalation mechanism of zinc ions into α-MnO2 by in situ X-ray diffraction (XRD in) more detail. Fig. 2a is charge-discharge profile for the first two succes sive cycles and Fig. 2b is the corresponding in situ X-ray XRD patterns during the cycling. In regions II and III, counter-diffusion between Mn2þ and Zn2þ ions occurs during the electrochemical process, leading to the emergence of a new phase. In regions I and IV, Zn2þ ions diffuse into/out of the 2 � 2 tunnel of α-MnO2, where only one single phase reaction
occur. The result shows that Zn-birnessite is not a direct reaction product of zinc insertion into α-MnO2, but was formed by the loss of the inter calated zinc ions and water molecules from the layers of buserite. Buserite crystallize has the channel width of about 10–11 Å, which is an important precursor of other types of manganese dioxide . In aqueous solution, Zn2þ ions are usually octahedrally coordinated with water molecules octahedrons to form [Zn(H2O)6]2þ . Owning to the high charge density of central divalent cation, the water molecules in the complex are strongly polarized, which causes hydrolysis to generate [Zn (H2O)6-h(OH)h](2 h)þ (h represents the degree of hydrolysis). Since the width of the buserite tunnel is large (about 11 Å), Zn2þ ions may move through the channel with [Zn(H2O)6-h(OH)h](2 h)þ so that the charge of Zn2þ ions is partly shielded. When the amount of Zn2þ ions is large, Zn2þ ions in layered MnO2 compounds adopt octahedral configurations on the manganese vacancy site coordinated with three oxygen atoms adjacent to vacancy sites and three water molecules inside the channel . When the amount of Zn2þ ions is small, the ions are tetrahedral with one water molecule above/below the manganese vacancies . It is known that the structure of buserite has three water layers in the channel, which may help to insert or remove of zinc ions. The large volumetric change between α-MnO2 and Zn-buserite can induce a large amount of residual structural stress during the electrochemical cycle, which leads to collapse of the layered structure during repeated cycles, ultimately resulting in decrease of capacity. After that, Lee’s  team also synthesized the α-MnO2 nanorod cathode by using a hydrothermal method through reduction of KMnO4 with NH4Cl and studied the role of pH evolution of aqueous zinc sulfate electrolyte. They found that Zn2þ ions precipitated on the surface of α-MnO2 and formed layered zinc hydroxide sulfate (Zn4(OH)6(SO4)⋅ 5H2O) (Fig. 2c) instead of intercalate into the tunnels of α-MnO2. The formation of Zn4(OH)6(SO4)⋅5H2O is dependent on the pH value of the solution. Therefore, they proposed a new reaction mechanism of RZIBs. During the discharge process, the electrochemical reduction of 4
C. Li et al.
Journal of Power Sources 449 (2020) 227596
manganese dioxide on the cathode produces an unstable trivalent manganese, Mn3þ (Mn4þ þ e →Mn3þ ) due to its high-spin electronic
KMnO4 and MnSO4⋅H2O as raw materials at 140 � C for 12 h. This battery exhibits high capacity of 225 mAh g 1 at 0.65 C, high rate capability of 100 mAh g 1 at 32.50 C and long term cycling stability (94% capacity retention after 2000 cycles at 6.50 C).
configuration (d4 ¼ t2g 3 g 1 ) [57,58]. This kind of Jahn-Teller cation is
inclined to experience a disproportionation (2Mn3þ →Mn4þ ðsÞ þ Mn2þ ðaqÞ), leading to manganese dissolve into electrolyte [59,60]. And the pH value of the electrolyte will increases, this phenomenon causes crystallization of zinc hydroxide sulfate from the electrolyte on the α-MnO2 surface. Moezzi et al. also reported that zinc hydroxide sulfate precipitated from aqueous ZnSO4 solution when the solution changed from acidic to neutral . Upon charging, due to the recombination of manganese on the cathode, the pH value of the electrolyte starts to decrease and the precipitate dissolve back into the electrolyte. The whole reaction can be written as: 3MnO2 þ 3Zn þ 5Zn2þ þ 2SO24 þ 16H2 O ↔ 3Mn2þ þ 2Zn4 ðOHÞ6 ðSO4 Þ⋅5H2 O↓ 
Their work reveals that it is important to construct a highly porous structure in the cathode to accommodate zinc hydroxide sulfate pre cipitates. Otherwise they may hinder the diffusion of Zn2þ and Mn2þ ions and further lead to increase of impedance. In the same year, Pan et al.  synthesized α-MnO2 nanofibres by a hydrothermal method. The length of α-MnO2 nanofibre extends to a few micrometres, with a diameter of about 50 nm. They presented that α-MnO2 is likely to react with a proton in water to form MnOOH (MnO2 þ Hþ þ e ↔ MnOOH), which reveals an alternative conversion reaction mechanism between MnOOH and MnO2 other than Zn2þ ion intercalation into MnO2. The Hþ ions react with MnO2 in aqueous solution, as a result, the sequent OH ions react with ZnSO4 and H2O to form a large flake-like ZnSO4[Zn (OH)2]3⋅xH2O and reach a neutral charge in the system. 2.1.2. β-MnO2 Earlier, Jiao et al.  synthesized mesoporous β-MnO2 with highly intense (110) plane orientation and found that a large amount of Liþ intercalates and deintercalates easily in its structure to form Li0.92MnO2. Su et al.  synthesized α-MnO2 and β-MnO2 nano-rods by hydro thermal method using (NH4)2S2O8 and MnSO4⋅H2O as raw materials, cationic surfactant cetyltrimethylammonium bromide (CTAB) as a soft template at 140 � C for 12 h. When applied β-MnO2 nano-rods as a cathode of sodium-ion batteries, it exhibits better electrochemical per formances such as good rate capability and cyclability than that of α-MnO2 nanorods, which ascribe to more compact tunnel structure of β-MnO2 nanorods. Therefore, β-MnO2 with large open tunnels also is one of the most promising cathode materials for RZIBs due to the similar ionic radius of Zn2þ (74 p.m.) with Liþ (76 p.m.). Islam et al.  prepared β-MnO2 nanorod with exposed (101) planes through rapid microwave-assisted hydrothermal method using KMnO4 and MnSO4 as raw materials at 200 � C for 10 min, and applied as the cathode material for RZIB for the first time. This β-MnO2 nanorod electrode exhibited a high discharge capacity of 270 mAh g 1 at 100 mA g 1, high rate capability (123 and 86 mAh g 1 at 528 and 1056 mA g 1, respectively), and long cycling stability (75% capacity retention with 100% Coulombic efficiency at 200 mA g 1) over 200 cycles. The results also showed that the cycle stability of β-MnO2 nanorods was significantly improved by adding MnSO4 in aqueous ZnSO4 electrolyte. Concerning the reaction mechanism of β-MnO2, they supposed that Zn2þ ions intercalated into β-MnO2 framework and formed spinel ZnMn2O4 Zn-inserted phase, meanwhile ZnSO4⋅3Zn(OH)2⋅5H2O deposited on the electrode surface. And during Zn2þ ions insertion, the lattice spacing of (101) plane of β-MnO2 undergoes a slight expansion. Therefore, tailoring crystal orientation for electrode material can promote facile ionic transports during electrochemical reaction, which is a promising strategy for the application of energy storage. Zhang et al.  designed a high-performing RZIB system based on zinc anode, β-MnO2 cathode, and 3 M Zn(CF3SO3)2þ0.1 M Mn(CF3SO3)2 aqueous electrolyte. The β-MnO2 nanorod cathode was synthesized by a hydrothermal method using
2.1.3. γ-MnO2 Zeng et al.  synthesized a sea-urchin shaped γ-MnO2 electrode using a facile hydrothermal method without employing any template or surfactant with mild conditions. This electrode delivered more than 100 mAh g 1 at a high current density of C/3 with high reversibility and good capacity retention after 20 cycles for lithium-ion battery. Mathew et al.  synthesized a self-assembled mesoporous γ-MnO2 electrode via ambient temperature redox synthesis at 200 � C, which registered an initial discharge capacity of 268 mAh g 1 with a well-defined plateau around 3 V in Li/MnO2 battery. In the field of sodium-ion batteries, Chae et al.  synthesized γ-MnO2 nanowire crystallites with diameters and lengths in the range of 2–3 and 25–40 nm by using the previous synthesis method. When employed in sodium-ion battery, this cathode presents initial discharge and charge capacities of 234 and 233 mAh g 1 with almost 100% Coulombic efficiency. Alfaruqi et al.  prepared mesoporous γ-MnO2 cathode with high surface area by a simple ambient temperature strategy followed by low-temperature annealing at 200 � C. When used in a RZIB, it delivers an initial discharge capacity of 285 mAh g 1at 0.05 mA cm 2 with a defined plateau at around 1.25 V vs Zn/Zn2þ. Moreover, the structural transformation of mesoporous γ-MnO2 cathode during electrochemical reaction was intensively investigated by in situ XRD and in situ Syn chrotron X-ray absorption near edge spectroscopy (XANES). The results indicate that the structural transformation of mesoporous γ-MnO2 cathode forms tunnel-type γ-ZnxMnO2 and layered-type L-ZnyMnO2 during the electrochemical reaction, and these phases with multi oxidation states coexist after complete electrochemical Zn-insertion. More specifically, a part of the orthorhombic γ-MnO2 is converted into spinel-type ZnMn2O4 in the initial stage. The 1 � 1 tunnel in the pyro lusite block of the γ-MnO2 structure is mainly converted into a spinel-type phase, which consistent with the result of Li-insertion in β-MnO2 . With the further progress of discharge reaction, the 1 � 2 tunnels in the domains that retain the parent orthorhombic structure become infiltrated and occupied by zinc, thus tending to expand the geometric dimension of the tunnels and form a new γ-ZnxMnO2 phase. During the later stages of discharge reaction, some of the fully inserted tunnels expand further and open up the structure as more Zn-insertion occurs, eventually forming a layered-type MnO2 with a larger d-spacing (7.26 Å). When the Zn-insertion is completed, the spinel-type ZnMn2O4, tunnel-type γ-ZnxMnO2, and layered-type ZnyMnO2 phases coexist and this process accompany by the reduction of manganese from Mn(IV) to the Mn(III) and Mn(II) states. During the subsequent charging or Zn-deintercalation process, the layered-type polymorph tends to become compressed and revert back to the parent orthorhombic lattice of γ-MnO2. The result of ex situ high resolution-transmission electron microscopy (HR-TEM) also confirms the structure transformation of γ-MnO2 during electrochemical reaction. 2.1.4. Akhtenskite MnO2 (ε-MnO2) Regarding the reaction mechanism of MnO2 in neutral or mild acidic aqueous electrolytes, there is still uncertain and remains controversial. Several works demonstrated that the capacity of MnO2 in aqueous electrolytes is induced by the reversible Zn2þ insertion/extraction [42, 48,51]. Lee et al. investigated the reaction mechanism of α-MnO2 cathode in an aqueous zinc sulfate electrolyte by monitoring structural changes. The result shows that Zn2þ ions mostly precipitate on the surface of the electrode or in the porosity between the particles to form zinc hydroxide sulfate, rather than intercalating into the tunnels of MnO2 . Pan et al. showed a different reaction mechanism of α-MnO2 cathode which supported the reversible Hþ insertion/extraction to form MnOOH . Sun et al.  prepared the binder free Akhtenskite MnO2
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Fig. 3. (a) Schematic illustration of the nanocrystalline MnO2 electrodeposited on carbon fiber paper (CFP) process, and the corresponding SEM images of CFP before and after electrodeposition. (b) Schematic illustration of the Zn/CFP battery in ZnSO4þMnSO4 aqueous electrolyte before MnO2 deposited on CFP. (c) Charge and discharge curves at different rates in first cycle. (d) Discharge curves of [email protected]
cathode in 0.2 M MnSO4 solution with or without ZnSO4 as electrolytes at 0.3 C between 0 and 0.8 V (vs Ag/AgCl) in a three electrode cell. Reproduced with permission from Ref. . Copyright 2017 American Chemical Society.
cathode by in situ electrodeposition of MnO2 on carbon fiber paper ([email protected]
) and designed a highly reversible RZIB in mild acidic ZnSO4þMnSO4 electrolyte. And they first proposed the mechanism of the consequent Hþ and Zn2þ insertion mechanism. The electrodeposited MnO2 has a nanocrystalline structure and the particle size is typically less than 10 nm. The small particles offer a relatively large electro de/electrolyte contact area and therefore tend to enhance the diffusion kinetics by reducing the diffusion pathway for electronic and ionic transport. Fig. 3a is the illustration of the nanocrystalline MnO2 elec trodeposited on carbon fiber paper (CFP) and Fig. 3b is a schematic diagram of the composition of this battery in ZnSO4þMnSO4 aqueous electrolyte. This [email protected]
cathode shows a considerably high ca pacity of 290 mAh g 1 at 0.3 C, close to the theoretical capacity of MnO2 (308 mAh g 1, based on molecular weight of MnO2 and 1 e transfer reaction). At the rate of 1.3C, it exhibits an initial discharge capacity of 260 mAh g 1 and maintains 150 mAh g 1 after 20 cycles. Even at a high rate of 6.5 C, [email protected]
cathode can provide a stable capacity of 50–70 mA h g 1 for 10000 cycles, the corresponding Coulombic effi ciency is nearly 100%. Fig. 3c is the charge and discharge curves of this battery at different rates in the first cycle. With the increase in charge and discharge rate, the voltage and capacity drop in the first voltage plateau (region I, ~1.4 V) are very small, whereas both the voltage and capacity in the second voltage plateau (region II, ~1.3 V) significantly declined, indicating that the reaction kinetics in region I is much faster than the reaction in region II. Results of galvanostatic intermittent titration technique (GITT) and electrochemical impedance spectroscopy (EIS) reveal that the total overvoltage in region II is 0.6 V, which is almost 10 times than that of in region I (0.08 V) and the charge transfer and diffusion resistance in the region II is much larger than the charge transfer and diffusion resistance in region I. Since the size of Hþ is much smaller than Zn2þ, they conclude that region I takes place Hþ insertion process, whereas the voltage plateau in region II is mainly attributed to the Zn2þ insertion. Electrochemical behavior of [email protected]
cathode in 0.2 M MnSO4 electrolyte without ZnSO4 further confirms this hypothesis (Fig. 3d). Since the absence of Zn2þ, the flat plateau of 1.3 V in region II
vanishes, only one sloped plateau from 1.8 to 1.35 V appear (Hþ insertion), which demonstrates that the main reaction in region II is caused by Zn2þ insertion. Ex situ XRD measurements are conducted on [email protected]
electrode after discharge to 1.3 and 1.0 V and maintain at 1.3 and 1.0 V for 24 h to identify the equilibrium phase in regions I and II. Typical MnOOH and ZnMn2O4 equilibrium phase are observed by ex situ XRD measurements further strongly support the mechanism that the [email protected]
cathode experiences Hþ insertion followed by Zn2þ insertion. 2.1.5. δ-MnO2 Based on previous researches of tunnel-type α- and γ-MnO2 poly morphs in RZIB, Alfaruqi et al.  turned their attention to the layered type δ-MnO2 polymorph with a large interlayer (~7.0 Å). They fabri cated a δ-MnO2 cathode with flake-like morphologies via the simple low temperature thermal decomposition of KMnO4. The Zn/δ-MnO2 battery assembled with the nano-flake δ-MnO2 cathode under atmospheric condition exhibits an open-circuit voltage (OCV) of about 1.49 V, discharge capacities as high as 250 mAh g 1 under a current density of 83 mA g 1 and a Coulombic efficiency of nearly 100% during 100 cycles. Furthermore, the reaction mechanism of the δ-MnO2 cathode was studied by using the ex situ XRD and inductively coupled plasma (ICP). The results reveal that the δ-MnO2 undergoes a structural trans formation to form spinel-type ZnMn2O4 with Mn (III) state and layered-type δ-ZnxMnO2 with Mn (II) phase. Nevertheless, no irrevers ible phases, such as MnOOH, Mn(OH)2, Mn3O4, Mn2O3 and ZnO are observed after the discharge reaction, which means there’s no side re actions occurring in the cathode. Han et al.  reported a new RZIB system based on δ-MnO2 (K0⋅11MnO2⋅0.7H2O) cathode, Zn metal anode and nonaqueous aceto nitrile-Zn(TFSI)2 electrolyte. The nanostructured K0⋅11MnO2⋅0.7H2O cathode material was synthesized using a low temperature water-based synthetic route. A great deal of research has been demonstrated that the nonaqueous acetonitrile-Zn(TFSI)2 electrolytes can support highly reversible Zn deposition behavior on a Zn metal anode (�99% of 6
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Fig. 4. (a) Cyclic voltammogram (CV) curves of Zn electrode in 1 M Zn(CF3SO3)2 at the scan rate of 0.5 mV s 1 between 0.2 and 2.0 V. (b) CV curves of Zn electrode in 1 M ZnSO4 at the scan rate of 0.5 mV s 1 between 0.2 and 2.0 V. (c) Schematic illustration of Zn2þ insertion/extrac tion in an extended three-dimensional ZnMn2O4 spinel framework. (d) Proposed Zn2þ diffusion pathway in ZnMn2O4 spinel without and with Mn vacancies. Reproduced with permission from Ref. . Copyright 2016 American Chemical Society.
Coulombic efficiency) with wide electrochemical window (up to 3.8 V vs. Zn/Zn2þ) [75–77]. This new RZIB system exhibits a high capacity of 123 mAh g 1 after 125 cycles at a current density of 12.3 mA g 1 with good reversibility (>99% Coulombic efficiency) and an operating voltage of 1.25 V (vs Zn/Zn2þ). The study results of transmission elec tron microscopy (TEM), element mapping and ex situ XRD analysis show that the layer-type δ-MnO2 cycles reversibly between the pristine ma terial and ZnxMnO2 (xmax ¼ ~0.2) when Zn2þ ions insert into the host material during discharging. At the same time, the Zn2þ ions insertion process accompanied by a competing side reaction to irreversible for mation of ZnO. However, the amount of ZnO does not apparently in crease during cycling, which indicate that it is not only from lattice breakdown, but may be partially derived from the reaction with water or a disproportionation reaction of ZnxMnO2 in the bulk. Thus, the whole reaction can be written as: xZn þ K0:01 MnO2 ⋅0:7H2 O ↔ Znx K0:01 y MnO2 þ yKþ þ 0:7H2 O
Mg1:8 Mn6 O12 ⋅ 4:8H2 O þ 1:2Zn2þ þ 2:4e ¼ Zn1:2 Mg1:8 Mn6 O12 ⋅4:8H2 O
2.2. Spinel ZnMn2O4 Spinel-type ZnMn2O4 has been investigated extensively as the anode materials for lithium-ion batteries [81,82]. ZnMn2O4 is also a promising candidate cathode material for aqueous RZIB because Liþ and Zn2þ have almost the same ionic radius. Knight et al.  investigated the chem ical extraction of Zn from the spinel ZnMn2O4 and found that the ideal spinel structure is not suitable as a RZIB cathode due to the large elec trostatic repulsion while the Zn2þ ions diffuse through the lattice. In order to reduce the electrostatic repulsion, they suggest creating va cancies to allow for easier Zn2þ ions diffusion in the structure through controlling synthesis conditions or additional treatments. Koketsu et al.  introduced plenty of charge-compensating titanium vacancies (22%) in anatase TiO2 through aliovalent ion doping to realize the �nchez et al. reversible insertion of multivalent ions (Mg2þ and Al3þ). Sa  studied the electrochemical insertion of Mg2þ into the cation-deficient mixed spinel oxide Mn2.15Co0.37O4. The cation va cancies in the mixed oxide offer a route for Mg2þ insertion with a maximum absorption of 0.23 Mg per mole of oxide. Inspired by the above works, Zhang et al.  reported cation-defective ZnMn2O4/carbon (60 wt% spinel and 40 wt% carbon) composite as cathode material of aqueous RZIBs. The composition of spinel in cation-defective ZnMn2O4/carbon can be written as ZnMn1.86Y0.14O4 (where the Y represents vacancy). The abundant cation vacancy character is caused by the mild solution-based synthesis (a low temperature of 180 � C and a short time of 3 h), which helps to form the ultrafine and nonstoichiometric spinels . They also investigated the electrochemical properties of ZnMn2O4/carbon in four mild acidic ZnCl2, ZnNO3, ZnSO4 and Zn(CF3SO3)2 aqueous electrolytes. Fig. 4a and b are CV curves of Zn electrode in aqueous electrolyte of 1 M Zn (CF3SO3)2 and 1 M ZnSO4. The results showed that Zn(CF3SO3)2 has better reversibility and faster kinetics of Zn2þ deposition/dissolution, which attributes to the bulky CF3SO3 anion lessening the number of water molecules around Zn2þ and the solvation effect, promoting Zn2þ migration and charge transfer.
2.1.6. Todorokite-type MnO2 Todorokite-type MnO2 is a new cathode material for RZIB and has the crystallographic structure with1-dimensional 3 � 3 tunnels through the b-axis, which is the largest tunnel among other tunnel-type MnO2 polymorphs (α-MnO2 with a [2 � 2] tunnel, β-MnO2 with a [1 � 1], γ-MnO2 with a mix of [2 � 1] and [1 � 1] tunnel and δ-MnO2 with [1 � ∞] tunnel). Many cations, including alkali, alkaline-earth, transitionmetal ions, and even post-transition metal ions and water molecules, can intercalate into this large tunnel, giving an approximate composition of M1�xMn6O12⋅3–4H2O (M ¼ Na, Ca, Mg, Ba, K etc.) . Wei et al.  synthesized α-, β-, γ-, and δ-types MnO2 with different tunnel structures and morphologies by a common liquid co-precipitation method based on the redox reactions of Mn4þ and Mn2þ. They studied the effect of the tunnel structures and morphologies on the storage properties of Zn2þ ions, and found that large tunnel structure is favorable to store Zn2þ ion. Lee et al.  synthesized todorokite-type MnO2 cathode by the hy drothermal treatment of layered Na-birnessite in a concentrated Mg-containing solution and investigated its structural and electro chemical properties. The todorokite-type MnO2 cathode for RZIB delivered a discharge capacity of 108 mAh g 1 at C/2 and good rate performance in the potential range of 0.7–2.0 V. Electrode reaction on the cathode can be written as: 7
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Previous studies on Li batteries have proved that higher salt con centration can reduce the water activity and water-induced side re actions, thereby enhancing cycle stability and kinetics in aqueous solutions [88,89]. For the Zn(CF3SO3)2 electrolyte (pH � 3.6) with concentration of 3 M, the O2 evolution potential was suppressed to 2.5 V. More importantly, there are no detectable side reactions in the working voltage window of aqueous RZIB (0.8–1.9 V). This cation-defective ZnMn2O4/carbon composite delivers initial specific charge and discharge capacities of 128 and 120 mAh g 1 at the current rate of 50 mA g 1 between 0.8–1.9 V. Even at a high current rate of 2000 mA g 1, the discharge capacity can reach to 72 mAh g 1. In addition, considerable capacity retention of 94% after 500 cycles at high rate of 500 mA g 1 is attained. They do some morphological studies on the cathode and anode after 50 cycles. The results reveal that the spinel nanoparticles of ZnMn2O4/carbon cathode are still firmly anchored on and uniformly composited with carbon, and Zn anode shows a dendrite-free and dense surface morphology. They suggest that the excellent electrochemical perfor mance of ZnMn1.86Y0.14O4 cathode is derived from the rich Mn va cancies, which benefit for Zn2þ diffusion in the spinel framework. Upon charging or discharging, Zn2þ ions extract or insert from the Zn–O tetrahedral sites of ZnMn2O4 spinel (Fig. 4c and d). And the electro chemical reaction can be written as ZnMn1:86 Y0:14 O4 ↔ Zn1 x Mn1:86 Y0:14 O4 þ 2xe þ xZn2þ (0 < x < 1), where x represents the number of reversible extraction of Zn2þ and maximum is 0.7 in their study. Wu et al.  reported a hollow porous ZnMn2O4 cathode for the green-low-cost aqueous RZIB. This cathode is synthesized through a solvothermal carbon template method firstly, followed by an annealing process at 600 � C for 4 h in air. The carbon microsphere template is prepared by using glucose as raw material at 180 � C. And the hybrid electrolyte was synthesized by dissolving zinc sulfate and manganese sulfate in deionized water. This system exhibits reversible discharge capacity of 106.5 mAh g 1 at 100 mA g 1 after 300 cycles without ca pacity decay. At the same time, it displayed a high capacity of 70.2 mAh g 1 at high current density of 3200 mA g 1, which can be attributed to the mesoporous structure and residual carbon distribution facilitating the charge transfer and shortening the ion diffusion path lengths. Overall, great advances have been made in synthesis technology and energy storage mechanism researches of manganese-based cathode materials. The various manganese-based cathode materials, such as α-MnO2, β-MnO2, γ-MnO2, ε-MnO2, δ-MnO2, todorokite-type MnO2 and Spinel ZnMn2O4 have been synthesized by using different synthesis technologies, including microemulsion, hydrothermal, low-temperature thermal decomposition, in situ electrodeposition, liquid co-precipitation method and solvothermal carbon template method. However, there are many drawbacks for these synthesis technologies that have not yet been resolved. So new synthesis technologies reducing the manufacturing costs need to be developed for ZIBs to become commercial products. For the reaction mechanism of Mn-based cathodes, there are still many missing details that are yet to be revealed, for example, the variation in the Mn oxidation state is still not clear. Especially the manganese-based cathode materials still suffer the problem of fast capacity decay during the cycling due to dissolution of Mn2þ from Mn3þ disproportionation into mild acidic aqueous electrolytes.
manganese-based oxide and the structural evolution by analyzing the Mn concentration in electrolyte solution and electrochemical perfor mances through inductively coupled plasma (ICP) and CV techniques. They found that adding 0.1 M MnSO4 additive into the mild ZnSO4 aqueous electrolyte can change the dissolution equilibrium of Mn2þ from the MnO2 electrodes, suppress continuous Mn2þ dissolution and greatly improves the capacity decay. Moreover, the MnSO4 additive in electrolyte the do not affect the redox reactions in the MnO2 electrode. This battery achieves a higher capacity of 260 mAh g 1 at current rates of 1C, excellent rate capability (207, 161 and 113 mAh g 1 at 2C, 5C and 10C) and excellent long cycle stability with high capacity retention of 92% after 5000 cycles at 5C. Adding conductive additives, surface coating and metal ion doping are also effective measures to solve these problems. Wang et al.  synthesized carbon-coated α-MnO2 nanoparticles (α[email protected]
) using maleic acid (C4H4O4) as a carbon source and applied as a cathode ma terial for aqueous ZIB. The test results show that the carbon coating on the electrode material not only increases the electrical conductivity and discharge capacity but also improves the electrode stability and capacity retention by preventing dissolution of manganese from the MnO2 during the electrochemical discharge reaction. Wu et al.  proposed highly reversible aqueous RZIB using graphene scroll-coated α-MnO2 nano wires as the cathode to increase the electrical conductivity and relieve the dissolution of the cathode material during cycling. This battery exhibited considerable specific capacity of 145.3 mAh g 1 at 3 A g 1 with high retention of 94% after 3000 cycles. Yadav et al.  reported the development of Cu2þ-intercalated layered MnO2 cathodes. Cu is used as an intercalant to improve the electrochemical properties of layered structure MnO2. This cathode exhibited a capacity of 617 mAh g 1 for over 900 cycles. In addition, Xu et al.  synthesized MnO2/ carbon nanotube (CNT) nanocomposites by a simple co-precipitation method for improving electrical conductivity and stabilize electrode. This MnO2/CNT anode delivered excellent Zn2þ storage properties (~400 mAh g 1 at 1 A g 1) and reversibility (~100% Coulombic effi ciency after 500 charge/discharge cycles). In short summary, these so lutions can not only efficiently suppress Mn dissolution from the MnO2 electrode but also improves the electrode stability and capacity retention. 3. Vanadium-based materials Vanadium (V)-based cathodes with different frameworks for RZIBs have advantages of stability and diversity by contrast with Mn-based cathodes. V–O coordination polyhedral can adopt different units and can be constructed by corner and/or edge sharing of these polyhedral. The frameworks of Vanadium-based cathodes allow for reversible Zn2þ intercalation/deintercalation . The V-based cathodes include va nadium pentoxide (V2O5), MxV2O5 (M ¼ Na, Ca, Zn, Mg, Ag, Li …) and other layered and tunnel-type vanadium-based compounds. 3.1. V2O5 V2O5 is found to be a successful candidate for storage of larger multivalent metal-ions, such as Mg2þ , Al3þ  and Zn2þ because its layered structure has the large spacing. Zhou et al.  synthesized low-cost V2O5 nanoparticle cathode by a wet chemistry method reported at 400 � C in air for 2 h. They investigated the influence of different type of the aqueous electrolytes (ZnSO4, Zn(CH3COO)2, Zn(NO3)2 and ZnCl2) on the electrochemical performances of this Zn/V2O5 system. The results show that the V2O5 nanoparticle cathode in 3 M ZnSO4 electrolyte delivered a high specific of 224 mAh g 1 at 100 mA g 1, and an excellent long-term cycling performance up to 400 cycles at 2 A g 1. The ZnSO4 electrolyte can achieve the better reversibility and faster kinetics of Zn deposition/dissolution . Hu et al.  develop a novel hybrid-ion battery system by using porous V2O5 as the cathode and metallic zinc as the anode as well as a new “water-in-salt” electrolyte (21 M lithium
2.3. Dissolution of manganese-based oxide Metal oxide cathodes generally suffer from the dissolution of metals during the battery operation because of the commonly used (slightly) acidic electrolytes. The technique used to monitor the dissolution of manganese-based oxide and the structural evolution has been researched widely. Some effective solutions to this problem including surface coating, electrolyte optimization, as well as composition tuning are proposed also. Pan et al.  monitored the dissolution of 8
C. Li et al.
Journal of Power Sources 449 (2020) 227596
that water molecules in oxide lattice layers act as coordinating and stabilizing molecules, which contribute to fast Zn2þ ion diffusion. Later, Yan et al.  investigated the critical role of structural H2O on Zn2þ intercalation into bilayer V2O5⋅nH2O (n � 1) in 3 mol L 1 Zn (CF3SO3)2 electrolyte in detail. The results show that the H2O-solvated Zn2þ possesses largely reduced effective charge, thereby reducing elec trostatic interactions with the host material framework and effectively promoting its diffusion. The XRD patterns (Fig. 5a) of V2O5⋅nH2O at different charge and discharge states show that Zn2þ ions are extracted from the interlayer during the charging process, and the interlayer spacing of bilayer V2O5 changes from 12.6 to 10.4 Å after charging to 1.3 V. There are two stages for the discharge process. The first discharge redox appears at about 1.1–0.8 V accompany with 0.3 mol Zn2þ ions intercalation. The second discharge redox happens in the voltage range of 0.6–0.4 V. It is found that a new phase with the interlayer distance of 13.5 Å is formed due to the intercalation of Zn2þ ions. Since the water-based shielding layer reduces the “effective charge” of Zn2þ and increases the distance between Zn2þ and the neighboring oxygen ions (r0), the interlayer distance of bilayer V2O5 increases from 10.4 to 13.5 Å due to Zn2þ intercalation. The results of the solid-state magic-angle-s pinning (MAS) nuclear magnetic resonance (NMR) also indicate that water is highly involved in the battery charge/discharge processes and plays an important role. Nam et al.  adopted the same strategy to introduce crystal water (~10 wt%) into the layered MnO2 cathode of aqueous RZIB. The interlayer crystal water can effectively screen the electrostatic interactions between Zn2þ ions and host framework to facilitate Zn2þ diffusion. It can also sustain the host framework for prolonged cycles, enhancing the rate and stable cycling performances.
Fig. 5. (a) XRD patterns of V2O5⋅nH2O at different charge and discharge states. Reproduced with permission from Ref. . Copyright 2017 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim. (b) Schematic illustration of the zinc-storage mechanism in the Na0.33V2O5 electrode. Reproduced with permission from Ref. . Copyright 2018 WILEY-VCH Verlag GmbH & Co. KGaA, Weinheim.
3.2. MxV2O5 (M ¼ Na, Ca, Zn, Mg, Ag, Li …) The above results show that water molecule intercalated into the interlayers of V2O5 can effectively stabilize their open-framework crystal structure to improve electrochemical performance of RZIBs. In addition, embedding large metallic ions to form the metal vanadate also is an effective method preventing structural collapse. Kundu et al.  synthesized single-crystal Zn0.25V2O5⋅nH2O nanobelts by microwave hydrothermal technique. The results show that interlayer metal ions and structural water in this layered oxide act as pillars, enhancing structural stability and cation migration during cycling. This Zn2þ intercalated cathode has high specific capacities (250–300 mA h g 1) and long-term cyclability (>1000 cycles) with 99% Coulombic efficiency at high cur rent rates of 15C (1C ¼ 300 mA g 1). Xia et al.  proposed a double-layered calcium vanadium oxide bronze (Ca0.25V2O5⋅nH2O) as aqueous RZIB intercalation cathode. Compared with Zn0.25V2O5⋅nH2O, the nanostructure Ca0.25V2O5⋅nH2O synthesized by using one-step hy drothermal method at 200 � C for 72 h offers larger CaO7 polyhedra, smaller molecular weight and density as well as higher electrical con ductivity. The Ca0.25V2O5⋅nH2O cathode delivers capacities of 340 and 289 mAh g 1 at 0.2 and 1 C, respectively. He et al.  presented a low-cost, safe, high capacity (367.1 mAh g 1 at a current density of 0.1 A g 1) and long life (with the capacity retention over 93% for 1000 cycles) aqueous RZIBs, which comprised of Na0.33V2O5 nanowire cath ode, 3 M Zn(CH3F3SO3)2 electrolyte, and zinc anode. Na0.33V2O5 nanowire cathode was prepared through a simple hydrothermal method. As for the Na0.33V2O5 electrode, Naþ intercalate into [V4O12]n layers and act as “pillars” to increase the stability of the tunnel structure upon ions insertion/extraction. They have demonstrated that the intercalation of sodium ions between the [V4O12]n layers can improve electrical conductivity through single nanowire device. The result shows that the conductivity of Na0.33V2O5 (5.9 � 104 S m 1) is apparently higher than that of pure V2O5 (7.3 S m 1). The morphology of Na0.33V2O5 is well maintained after 1000 cycles and only little variety of the amount of vanadium and sodium elements are captured in the electrolyte after different cycles. Besides, the results of inductively coupled plasma optical emission spectroscopy analysis (ICP-OES) show
bis(trifluoromethane sulfonyl)imide (LiTFSI) and 1 M Zn(CF3SO3)2). The “water-in-salt” electrolyte is able to retard the hydrogen and oxygen evolution at a high electrochemical window (~3.0 V) in this Zn/V2O5 battery [99,100]. The porous V2O5 cathode delivers a high discharge capacity of 238 mAh g 1 at 50 mA g 1 and 80% of the initial discharge capacity can be retained after 2000 cycles at a high current density of 2000 mA g 1. More importantly, the discharge platform increase from 0.6 to 1.0 V. Moreover, they confirmed the intercalation reaction mechanism of Zn2þ ions in V2O5 by using ex-situ X-ray photoelectron spectroscopy (XPS) and HR-TEM test. The results show that Zn2þ ions can be successfully intercalated into V2O5 after discharged to 0.2 V, which leads to the increase of (200) lattice spacing (2.43%), but not all the Zn2þ ions can be de-intercalated after recharging to 1.6 V. They assume that the captured Zn2þ ions may act as the interlayer pillars and stabilize the layered structure of V2O5 during the charge/discharge processes, which is similar to the effects of pre-intercalated metal ions (Liþ, Naþ, Kþ, Zn2þ …) in V2O5 . This work provides an effective method to enhance the energy density and long-term cycling stability of zinc-ion based aqueous batteries. Senguttuvan et al.  synthesized a hydrated bilayered V2O5 (BL-V2O5) cathode with a large gallery spacing of 11–13 Å by electro chemical deposition on carbon substrate with good porosity. The OCV of this Zn/V2O5 battery in nonaqueous acetonitrile (AN)-Zn(TFSI)2 elec trolyte is 1.42 V vs Zn2þ/Zn, and approximately 0.59 mol of Zn2þ can be inserted per mole of V2O5, which leads to reduced gallery spacing. This phenomenon of gallery spacing was demonstrated by the fact that Mg2þ ions can be effectively intercalated into interlayer spacing of BL-V2O5 . The BL-V2O5 cathode delivers stable capacities of �170 mAh g 1 for 120 cycles with a Coulombic efficiency of 83.7% at C/10. Even at a high rate of 20 C, it also exhibits a capacity of 130 mAh g 1. The Ca pacity decay at high rate can be attributed to morphological changes, electrochemical polishing phenomena, and loss of electronic contact of the active material with the carbon substrate . They also speculate 9
C. Li et al.
Journal of Power Sources 449 (2020) 227596
that the sodium content is stable at different states. In other words, the sodium ions do not change during charge/discharge process, indicating that the tunnel framework of Na0.33V2O5 is maintained by Naþ between the [V4O12]n layers, which prove the “pillars” effect of sodium ion. Fig. 5b shows the storage mechanism of zinc ion in the Na0.33V2O5 electrode. Shan et al.  constructed a Zn/Ag0.4V2O5 system and first demonstrated the combination displacement/intercalation (CDI) reac tion mechanism in aqueous RZIBs. The CDI reaction has been well-established in lithium-ion batteries, as observed in CuTi2S4 , Ag2VP2O8 , Ag2VO2PO4 , etc. The Zn2þ/Agþ displacement reaction occurs during Zn2þ insertion/extraction into/from the Ag0.4V2O5 structure. During discharge reaction, Zn2þ ions insert into host material to replace the Agþ sites and form a new Zn2(V3O8)2 phase. At the same time, Agþ is reduced to Ag0 to form the metallic Ag0 network in cathode. During charge reaction, most of the Zn2þ ions are extracted from the electrode, and the Zn2(V3O8)2 is transformed back to Ag0.4V2O5. In this process, small amount of Ag0 cannot be oxidized to Agþ, with a highly conductive Ag0 matrix remaining within the elec trode. As a result, the Ag0.4V2O5 cathode performs excellent rate capa bility as well as long-term cycling performance (stable capacity of 144 mAh g 1 after 4000 cycles at 20 A g 1). The CDI reaction of Zn2þ storage in Ag0.4V2O5 provides multi-electron charge transfers and highly conductive Ag0 matrix enables outstanding electrochemical perfor mance (stable capacity of 144 mAh g 1 after 4000 cycles at 20 A g 1). They also observed the similar phenomenon upon Zn2þ insertion/ extraction into/from the structure of copper pyrovanadate (Cu3(OH)2 V2O7⋅2H2O) in 3 M ZnSO4 electrolyte . In this material, the inserted Zn2þ ions not only drive the reduction of Cu2þ to Cu0 nano particles, but also accompany the phase transition process from Cu3(OH)2V2O7⋅2H2O to Zn0.25V2O5⋅H2O (Zn2þ replace Cu2þ) upon discharge. And during the charge process, the mixed phases of Zn0.25V2O5⋅H2O and Cu0 turn back to Cu3(OH)2V2O7⋅2H2O structure upon Zn2þ extraction. Ming et al.  also found CDI reaction in layered MgxV2O5⋅nH2O cathode. Their aqueous RZIBs system consists of MgxV2O5⋅nH2O cathode, zinc foil anode and 3 M Zn(CF3SO3)2 electro lyte. But different from CDI reaction in Ag0.4V2O5, the deintercalated Mg2þ in MgxV2O5⋅nH2O is found to deposit on Zn anode upon charge, then dissolved back in the electrolyte and served as the interaction cation along with Zn2þ ions upon discharge. The overall reaction can be written as: Zn0:3 Mgx V2 O5 þ zZn ↔ Znðzþ0:3Þ Mgx V2 O5
Zn3V2O7(OH)2⋅2H2O , Mo2.5þyVO9þz , VO1.52(OH)0.77 , LiV3O8 , H2V3O8 , Na2V6O16⋅1.63H2O , NaV3O8⋅1.5H2O , K2V8O21 , Na5V12O32 , etc.) have also been used as cathode materials for aqueous RZIBs because of their open-framework crystal structure and multiple oxidation states of va nadium. For example, in He’s  work, a H2V3O8 nanowire cathode with large interlayer spacing was synthesized through one-step hydro thermal method. This cathode was used in Zn(CF3SO3)2 aqueous elec trolyte, exhibiting the capacity of 423.8 mAh g 1 at 0.1 A g 1, and excellent cycling stability with a capacity retention of 94.3% over 1000 cycles. In H2V3O8 structure, V5þ and V4þ coexist with the ratio of 2:1, and the mixed valence of vanadium contributes to the improvement of electrochemical performance compared with other vanadium oxides . Hu et al.  synthesized a highly durable Zn/Na2 V6O16⋅1.63H2O nanowire cathode by a hydrothermal method. This cathode delivers a high specific capacity of 352 mAh g 1 at 50 mA g 1, and exhibit a capacity retention of 90% over 6000 cycles at 5000 mA g 1 in aqueous Zn(CF3SO3)2 electrolyte for aqueous RZIBs. Fang et al.  designed a highly reversible surface-oxided vana dium nitride (VNxOy) cathode material for aqueous RZIB, which com bines the insertion/extraction reaction and pseudo-capacitance-liked surface redox reaction mechanism. The energy storage of VNxOy cathode is not only accomplished by the typical cationic (Zn2þ and Hþ) de-/in tercalation accompanied by reversible cationic redox reaction (V3þ ↔ V2þ), but also provided by the release/uptake of anions (OH ) on the VNxOy surface with reversible anionic (N3 ↔ N2 ) redox, which are mainly responsible for the high reversibility and no structural degra dation of VNxOy. Therefore, the electrochemical reaction mechanism of VNxOy electrode can be summarized as below: � VN þ mZn2þ þ nHþ þ ð2m þ nÞe ↔ Znm Hn VN Insertion reaction  VNx Oy þ nOH ↔ VNx Oy
ðOHÞn þ ne
ðSurface redox reactionÞ
Such a novel energy release/storage mechanism significantly en hances the performance of Zn/VNxOy system in mild aqueous ZnSO4 electrolyte with an ultra-high-rate capability of 200 mA hg 1 at 30 A g 1 and superior long-term cyclic stability after 2000 cycles at 20 A g 1, which demonstrates great promise for potential applications in gridscale energy storage. The results show that the layered and tunneltype vanadium-based cathode materials with large interlayer spacing can improve effectively electrochemical stability of aqueous RZIBs.
4. Prussian blue analogues (PBAs)
Yang et al.  synthesized a new LixV2O5⋅nH2O cathode of RZIBs via a one-step hydrothermal method and followed by annealing process at 250 � C in air. The calculated result of XRD shows that the intercalation of Liþ into the interlayer of V2O5⋅nH2O further enlarges the interlayer distance of (001) face (13.77 Å), which is larger than that (001) face of V2O5⋅nH2O (12.00 Å). The large interlayer spacing facilitates the Zn2þ diffusion effectively, leading to improved electrochemical performance. The electrode delivers stable capacity of 232 mAh g 1 after 500 cycles at 5 A g 1. And a superior discharge capacity of 192 mAh g 1 after 1000th cycle can be obtained at 10 A g 1. Most importantly, the electrode maintains stable capacities and voltage platforms at the current densities between 0.5 and 10 A g 1 under extreme conditions (high and low testing temperatures). A high capacity of 149 mAh g 1 is achieved after 800 cycles with the capacity retention of 96.1% at 50 � C, and there is no capacity fading up to 2800 cycles at 0 � C under current density of 10 A g 1, which indicates the excellent temperature adaptability and poten tial practical application of LixV2O5⋅nH2O cathode.
Prussian blue analogues (PBAs) have large open-framework struc tures and a general formula of AxM [M’ (CN)6]y⋅nH2O (A ¼ metal ions; M ¼ Fe, Ni, Mn, V, Mo, Cu, Co; M’ ¼ Fe, Co, Cr, Ru). They belong to the Fm-3m space group with a face centered cubic structure, two metal ions (M and M0 ) are linked together by cyanide (CN) ligands . Due to the properties of non-toxic, inexpensive, easy to synthesize and open-framework structure, PBAs have already proven to be good host materials for monovalent metal-ion batteries (Liþ, Naþ, and Kþ) [129–131] as well as for multivalent metal-ion batteries (Mg2þ, Al3þ and Zn2þ) [132,133]. Zhang et al.  synthesized a rhombohedral Zn3[Fe (CN)6]2 (ZnHCF) cathode by using high temperature co-precipitation method and explored the cycling stability of ZnHCF in different elec trolytes (0.5 M Na2SO4, 0.5 M K2SO4, 1 M ZnSO4). When ZnHCF cathode is subjected to be cycled in Na2SO4 and/or K2SO4 electrolytes, the color of electrolytes changes from colorlessness to light yellow, while ZnSO4 electrolyte remain colorless during the cycling. The change of CV and color show the dissociation of ZnHCF in Na2SO4 and K2SO4 electrolytes to produce [Fe(CN)6]3 or [Fe(CN)6]4 . In order to confirm the exis tence of [Fe(CN)6]3 or [Fe(CN)6]4 , the electrolytes are analyzed by Ultraviolet–visible spectroscopy. There are three characteristic absorp tion bands of [Fe(CN)6]3 at 260 nm, 302 nm and 420 nm in both
3.3. Other vanadium-based materials In addition to the cathode materials mentioned above, other layered and tunnel-type vanadium-based compounds (such as 10
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Fig. 6. (a,b) SEM images of initial Zn deposits and after 100 cycles. (c) XRD patterns of initial Zn deposits and after 100 cycles. (d) Schematic demonstration of the insertion of Zn2þ ions in FeFe(CN)6. (e) FT-IR of fully charged and discharged FeFe(CN)6. Reproduced with permission from Ref. . Copyright 2016 American Chemical Society.
Na2SO4 and K2SO4 electrolytes, but no absorption bands in ZnSO4 electrolytes . Besides, [Fe(CN)6]3 (or [Fe(CN)6]4 ) can react with Fe2þ (or Fe3þ) ions to form insoluble (or soluble) Prussian blue Fe3[Fe (CN)6]2 (or KFeFe(CN)6). After adding FeSO4 solution into three elec trolytes, the colors of Na2SO4 and K2SO4 electrolytes quickly change from light yellow to blue, but ZnSO4 electrolyte remains colorless. Above results show that ZnHCF undergoes dissociation upon cycling in aqueous Na2SO4 and K2SO4 electrolytes, but is quite stable in aqueous ZnSO4 electrolyte. Mantia et al.  synthesized a copper hexacyanoferrate (CuHCF) nanopowder cathode by a co-precipitation method. This CuHCF cathode
in the ZnSO4 electrolyte yields an average voltage of 1.73 V. But ZnSO4 electrolyte has hydrogen evolution near the surface of the zinc electrode and the formation of zinc oxide, which block the surface and subse quently decrease Zn2þ ions diffusion. To avoid these intrinsic problems, Hong et al.  synthesized K0.86Ni[Fe(CN)6]0.954(H2O)0.766 nano particles by a simple precipitation method and studied the electro chemical performances of RZIB using K0.86Ni[Fe(CN)6]0.954(H2O)0.766 as cathode and zinc metal as anode in an organic electrolyte (acetonitrile (AN) contained 0.5 M Zn(ClO4)2). This battery exhibits an excellent reversible discharge capacity of 55.6 mAh g 1 and a discharge voltage of 1.19 V (vs. Zn2þ/Zn) at a rate of 0.2 C. The results show that the organic Fig. 7. (a) Basic Chevrel phases’ crystal struc ture: three types of cavities between Mo6S8 blocks. The face-sharing pseudocubes of cavities 1 and 2 form the channels in direction c (one of three equivalent directions in rhombohedral crystals). Reproduced with permission from Ref. . Copyright 2009 American Chemical Society. (b) Cyclic voltammogram behaviors of Na3V2(PO4)3/Zn at a scan rate of 0.1 mV s 1. (c) Schematic representation for phase transition of Na3V2(PO4)3 cathode during cycling. Repro duced with permission from Ref. . Copy right 2016 Elsevier Ltd.
C. Li et al.
Journal of Power Sources 449 (2020) 227596
electrolyte system also provides a high zinc cycling efficiency (>99.9%) than the aqueous system (~80%), but the formation of dendritic zinc seems to be unavoidable after cycles in this organic electrolyte. Developing biodegradable and biocompatible ionic liquid is an alternative strategy to overcome these drawbacks of organic electrolyte, such as dendritic zinc and eco-toxicity Liu et al.  prepared FeFe (CN)6 nanoparticle cathode by a solution precipitation method and designed a FeFe(CN)6/zinc RZIB with a cheap and green bio-ionic liq uid-water mixture electrolyte contained choline acetate of 30 wt%. The electrochemical cycling behavior of the Zn anode was investigated by using scanning electron microscopy (SEM) and XRD (Fig. 6a–c). By comparing SEM images (Fig. 6a and b) of initial Zn deposits and after 100 cycles, there are some very minor changes in morphology, which shows that the Zn anode has high stability in this electrolyte during the cycling. XRD results of the Zn anodes in Fig. 6c show only the diffraction peaks of Zn even after 100 charge/discharge cycles, further indicating the high stability of the Zn anode in bio-ionic liquid-water mixtures. They also studied electrochemical insertion and extraction of Zn2þ ions in FeFe(CN)6 cathode. The schematic demonstration of the insertion of Zn2þ ions in FeFe(CN)6 is shown in Fig. 6d. According to the result of Fourier Transform infrared spectroscopy (FT-IR) (Fig. 6e), there are peaks at 2183 and 2106 cm 1 in fully charged cathode (red curve), which attribute to the cyanide stretching vibration mode, ν(CN) of Fe (III)Fe(III)(CN)6 and Fe(III)Fe(II)(CN)6 . In the discharged state (black curve), these peaks shift to a lower wavenumber of 2168 and 2067 cm 1 and change their relative intensities, indicating that Zn2þ ions insert into FeFe(CN)6 and Fe(III) is reduced to Fe(II). The insertion of Zn2þ ions in PBAs is also confirmed by Energy-Dispersive X-ray spectroscopy (EDX), the result shows a Fe to Zn molar ratio of ~3:1 in fully discharged FeFe(CN)6, further proves the insertion of Zn2þ ions in cathode material.
6. Polyanionic materials NASICON-typed polyanionic materials possess extremely stable framework structure, large channel and plenty of vacancies, which can be used as Zn2þ ions storage guests for improving ionic diffusion capa bility and long cycle stability [147,148]. NASICON-typed Na3V2(PO4)3 (NVP) as host material for Naþ ions have been widely studied [149,150]. Huang et al.  obtained NVP nanoparticles by hydrothermal route followed by post calcination and first applied as intercalation host for divalent cations. They developed a new and eco-friendly RZIB by using NVP as cathode, zinc as anode and Zn(CH3COOH)2 as aqueous electro lyte. This aqueous battery delivers a reversible capacity of 97 mAh g 1 at 0.5 C and retains 74% capacity after 100 cycles. Meanwhile, the battery can be charged and discharged at high rate up to 10 C and the specific discharge capacity is 58 mAh g 1. Fig. 7b is CV behaviors of this system at a scan rate of 0.1 mV s 1. The oxidation peak in the first cycle at about 1.46 V vs. Zn2þ/Zn corresponds to Naþ ions deintercalation from NVP. The redox pair peaks during subsequent cycles appear at about 1.05 and 1.28 V, which can be attributed to Zn2þ ions deintercalate/intercalate from/into NVP cathode. As for the intercalation mechanisms of Zn2þ ions, they proposed that the NVP phase transform to NaV2(PO4)3 during charging accompany by the oxidation from V3þ to V4þ. When dis charging, Zn2þ ions insert into the NaV2(PO4)3 framework to form new ZnxNaV2(PO4)3 phase and V4þ is reduced back to V3þ. After recharging, V3þ is oxidized to V4þ accompanied by extraction of Zn2þ ions. The phase transition of Na3V2(PO4)3 cathode during cycling is shown in Fig. 7c. Na3V2(PO4)2F3 (NVPF) is another NASICON-typed cathode material and presents more stable structure than NVP because of the strong af finity of F atoms toward the surroundings [152,153]. Li et al.  first reported NVPF as a Zn intercalation cathode in 2 M Zn(CF3SO3)2 elec trolyte for RZIB. The Zn storage mechanism is similar to NVP cathode, NVPF is initially converted into Na2V2(PO4)2F3, and then 0.5 Zn2þ ions are inserted into Na2V2(PO4)2F3 to form Zn0.5Na2V2(PO4)2F3, after which Zn2þ ions are reversibly shuttled back and forth between Zn0.5Na2V2(PO4)2F3 and Na2V2(PO4)2F3. Interestingly, they fabricate a carbon film functionalizing Zn anode by rolled 80 wt% carbon black (super P) and 20 wt% PTFE into thin carbon film (thickness, ~0.1 mm) and placed on the surface of a Zn foil. The carbon film can change the deposition behavior of Zn and inhibit the dendritic Zn growth. There are large pieces of Zn dendrites perpendicularly grow and accumulate on the surface of Zn foil after 200 cycles (400 h). While much small and rela tively homogeneous distribution of Zn plates tend to parallel growth on the surface of Zn anode with carbon film. Due to the stable structure of NVPF and carbon film functionalizing Zn anode, this RZIB exhibits a high voltage of 1.62 V and remarkable cyclability of 95% capacity retention over 4000 cycles at 1 A g 1.
5. Chevrel phase Chevrel phase MxMo6T8 (M ¼ metal, T ¼ S, Se, or Te) also is a promising material for RZIBs because of its unique crystal structure. Fig. 7a shows a basic crystal structure of Chevrel phase: three types of cavities between Mo6S8 blocks (or Mo6-octahedral clusters inside anion cubes). The face-sharing pseudocubes of cavities 1 and 2 form the open three-dimensional channels in direction c (one of three equivalent di rections in rhombohedral crystals). Cavities 1 and 2 are available for cations insertion but cavity 3 not allows the occupation due to the strong repulsion between Mo atoms and inserting cations [140,141]. Chevrel phase compounds can accommodate various cations, such as mono valent (Liþ, Naþ) as well as divalent (Zn2þ, Cd2þ, Co2þ, Mg2þ) at ambient temperatures and have outstanding capability [142–144]. Chae et al.  researched the properties of the ZnxMo6S8 (x ¼ 1, 2) Chevrel phases, which prepared by electrochemical insertion of Zn2þ ions into Mo6S8. The Mo6S8 was first prepared via the chemical extraction of Cu ions from Cu2Mo6S8 synthesized via a solid-state reac tion for 24 h at 1000 � C. They find that the processes of Zn2þ ions insertion into Mo6S8 in different potential regions involve two steps. The first step occurs at higher-voltage region (around 0.45–0.50 V in CV) corresponding to the formation of ZnMo6S8 from Mo6S8. The second step occurs at a potential of around 0.35 V in CV, which defines the further reduction to form Zn2Mo6S8 from ZnMo6S8. Cheng et al.  synthe sized Chevrel phase Mo6S8 nanocubes through an intermediate com pound of Cu2Mo6S8, and acid leaching of Cu2þ ions and applied as the electrode material for RZIB. The sizes of Mo6S8 range from 20 to 150 nm with an average size of ~100 nm. This Mo6S8 host can host Zn2þ ions reversibly in both aqueous and nonaqueous electrolytes with specific capacities around 90 mAh g 1, and exhibits remarkable intercalation kinetics and cyclic stability.
7. Metal disulfides Layered metal disulfides, such as VS2  and MoS2 , have attracted tremendous attention as electrode materials for energy storage and conversion. The unique layered structure bonded by weak van der Waals’ forces in these materials promotes the mass transport of various charge carriers and can also accommodate the volume variations during intercalation of ions. He et al.  synthesized VS2 nanosheets by hydrothermal route and used VS2 nanosheets as cathode for aqueous RZIB. VS2 belongs to hexagonal system and the interlayer spacing is 5.76 Å. Their results demonstrate that the interlayer space of VS2 can self-adapt to the intercalation of Zn2þ with an expansion along the c-axis (only 1.73%) and a slightly shrink along the a- and b-axes. Insertion of Zn2þ ions into the interlamination of VS2 layer during the discharge can be divided into two steps. First, the phase change from VS2 to conductive Zn0.09VS2 occurs in the voltage range of 0.82–0.65 V, and the subsequent phase transition from Zn0.09VS2 to Zn0.23VS2 occurs in the voltage range of 0.65–0.45 V. In charging process, Zn2þ ions deintercalate from 12
C. Li et al.
Journal of Power Sources 449 (2020) 227596
for application in RZIBs. 8. Organic materials Organic cathode materials also are very attractive for RZIBs because of its unique advantages, such as flexible synthesis, lightweight, low cost, abundant resource and benign to the environment . Some organic quinone compounds have offered an interesting alternative to inorganic cathode materials for nonaqueous lithium and sodium ion batteries, but those batteries suffer fast capacity fading due to the dissolution of active materials in organic electrolytes . Applying quinone electrodes in aqueous batteries makes it possible to achieve stable electrochemical performance because quinones are barely soluble in aqueous electrolytes [161,162]. Zhao et al.  reported an aqueous RZIB with organic calix quinone (C4Q) cathode, Zn foil anode and 3 M Zn(CF3SO3)2 electrolyte. The C4Q cathode with open bowl structure and eight carbonyls was synthesized by using calix arene as a pre cursor and green p-aminobenzoic acid as a major component of folic acid – O double . The active centers of C4Q cathode are carbonyls (C– bond) in para-position, but the ortho carbonyls in C4Q cathode would cause larger steric hindrance for Zn2þ ions reactions, thus showing poor electrochemical performance. They also investigated the electro chemical performance distinction of C4Q cathode between filter paper separator and cation-selective membrane (Nafion) separator. The result reveals that the batteries with the Nafion membrane show higher stable cycling performance (93% capacity retention after 100 cycles). The uptake of Zn2þ ions will ionize the C4Q to form ZnxC4Q during dis charging. Then, the dissociation of ZnxC4Q to Zn2þ and C4Q2x makes it more soluble than C4Q. The dissolved C4Q2x in electrolyte can pass through the filter paper and react with zinc forming a by-product on the anode side, which causes the decline of capacity. Therefore, the batteries with the Nafion membrane show higher stable cycling performance because of the prevention of anions from crossing. Kundu et al.  presented another tetrachloro-1,4-benzoquinone (p-chloranil) organic cathode for aqueous RZIB. This p-chloranil mate rial hold together by weak intermolecular van der Waals force, posing only a modest Coulomb repulsion to the diffusing cations, which is facile and reversible for the intercalation of hard divalent cations. Fig. 8b and c shows the fully relaxed structure of pure p-chloranil and Zn2þ inserted p-chloranil, respectively. Interestingly, malleable lattice of p-chloranil allows a squeezing reorientation to make pathways for incoming Zn2þ by increasing the O–O distance and decreasing the Cl–Cl distance, which driven by the insertion of Zn2þ ions. In other words, the reorientation can be called as the rotation of stacked chloranil columns. The coordi nation of Zn2þ with two O and Cl of two chloranil molecules of adjacent columns produces atomic distances change, resulting in the accommo dation of Zn2þ ions in a slightly distorted tetrahedral environment. The structural flexibility facilitates a high capacity of �200 mAh g 1 with a very small voltage polarization of 50 mV in a flat plateau around 1.1 V. Porous crystalline covalent organic frameworks (COFs) have been widely explored as host materials for monovalent ions (Hþ, Liþ, Naþ) in energy storage system due to its structural tunability, well-defined porosity, and high chemical stability. Kurungot et al.  first demonstrated hydroquinone (HqTp) based COF acting as cathode ma – O and N–H functionalities in polymers terial for aqueous RZIB. The C– are capable of coordinating Zn2þ ions in electrochemical system. Be sides, HqTp possesses crystalline honey-comb structure with a unique pore size of 1.5 nm, which further boosts the movement of Zn2þ ions through the entire organic cathode. In their works, the efficient – O (O⋯Zn, ~2.0 Å) inter-layer interaction of divalent Zn2þ ions with C– and N–H (N⋯Zn, ~2.0 Å) from the adjacent layers provides an excellent discharge capacity of 276 mAh g 1 at 125 mAg 1 in an operating po tential of 0.2–1.6 V vs Zn/Zn2þ. Wang et al.  first applied 1,4,5, 8-naphthalene diimide (NTCDI) as cathode material for aqueous RZIB. The highly activated NTCDI is synthesized by dissolving 1,4,5,8-naph thalenetetracarboxylic dianhydride (NTCDA) in ammonia solution to
Fig. 8. (a) Schematic illustration of Zn2þ insert into pristine MoS2. Reproduced with permission from Ref. . Copyright 2019 American Chemical Society. (b) Structural models of p-chloranil and (c) Zn-p-chloranil (Zn⋅C6Cl4O2) as ob tained from density functional theory (DFT) structural optimization. The curved arrows in (b) show the direction of the rotation of the pchloranil molecular columns upon Zn2þ insertion. Color code: C (brown), Cl (green), O (red), and Zn (gray). Reproduced with permission from Ref. . Copyright 2018 American Chemical Society. (For interpretation of the references to color in this figure legend, the reader is referred to the Web version of this article.)
Zn0.23VS2 and gradually change back to VS2 phase. The electrochemical reaction in the VS2 cathode can be summarized as below: 
VS2 þ 0:09Zn2þ þ 0:18e ↔ Zn0:09 VS2
Zn0:09 VS2 þ 0:14Zn2þ þ 0:28e ↔ Zn0:23 VS2
MoS2 can reversibly intercalate Li and Na ions but does not readily intercalate Zn2þ ions with higher valence. Liang et al.  realized fast Zn2þ diffusion in MoS2 through simple interlayer spacing and hydro philicity engineering which achieved by oxygen incorporation (MoS2–O). The smaller size of O atoms (48 p.m. vs 88 p.m. of S atoms) and the shorter Mo–O bonds (1.86 Å vs 2.42 Å of Mo–S bonds) weaken the van der Waals interactions between the two adjacent S layers, therefore resulting in the interlayer spacing to increase from 6 to 9 Å. In addition, the oxygen incorporation improves the hydrophilicity, lowers the Zn2þ intercalation energy. The schematic demonstration of the insertion of Zn2þ ions in pristine MoS2 is shown in Fig. 8a. In 3 M Zn (CF3SO3)2 electrolyte, the RZIB based on MoS2–O cathode delivers a discharge capacity of 232 mAh g 1 at 0.1 A g 1, which is much higher than that of MoS2 based RZIB (21 mAh g 1). More importantly, the Zn2þ diffusivity in MoS2–O is boosted by 3 orders of magnitude compared with unmodified MoS2. Xu et al.  prepared the defect-rich MoS2-x nanosheets by a simple hydrothermal process followed by heat treat ment and applied defect engineering to enhance the electrochemical activity of MoS2 electrode. These MoS2-x nanosheets show a preferential insertion of Zn ions into sulfur vacancies, allowing a much greater ca pacity to be obtained compared to pure MoS2. The electrochemical re action in MoS2-x cathode can be written as follows: þ
þ 0:36Zn2þ þ 0:728e ↔ Zn0:36 MoS2
The phase transition from MoS2-x to Zn0.36MoS2-x occurs in the discharge process, and Zn2þ ions extract from Zn0.36MoS2-x to form the MoS2-x phase gradually during charging process. This defect-rich MoS2-x electrode provides a high reversible capacity of 135 mAh g 1 at 100 mA g 1. Moreover, the MoS2-x can deliver a high reversible capacity of 88.6 mAh g 1 with capacity retention of 87.8% at 1000 mA g 1 after 1000 cycles. The defect-rich MoS2-x cathode displays excellent electro chemical performance, making it a highly promising cathode material 13
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Table 4 Synthesis methods and synthesis conditions of various cathode materials with different structures. Cathode material
α-MnO2 nanorod α-MnO2 nanorod α-MnO2 nanorod α-MnO2 nanorod α-MnO2 nanorod α-MnO2 nanofibre α-MnO2 nanowire
β-MnO2 nanorod β-MnO2 nanorod γ-MnO2 nanowire ε[email protected]
(Carbon fiber paper) δ-MnO2 nanoflake Todorokite MnO2 nanorod Spinel ZnMn2O4 microsphere MnO2 nanorod/CNT (Carbon nanotube) V2O5 microplate V2O5/CFS (Carbon foam substrate) Zn0.25V2O5⋅nH2O nanobelt Ca0.25V2O5⋅nH2O nanobelt Na0.33V2O5 nanowire Ag0.4V2O5 nanobelt Cu3(OH)2V2O7⋅2H2O nanosheet MgxV2O5⋅nH2O nanobelt LixV2O5⋅nH2O nanosheet H2V3O8 nanowire Na2V6O16⋅1.63H2O nanowire Zn3[Fe(CN)6]2 particle CuHCF nanopowder K0.86Ni[Fe(CN)6]0.954(H2O)0.766 nanoparticle FeFe(CN)6 nanoparticle ZnxMo6S8 particle Mo6S8 nanoparticle Na3V2(PO4)3 nanoparticle
Microemulsion method Microemulsion method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Microwave-assisted hydrothermal method Hydrothermal method Redox reaction process Electrodeposition method Thermal decomposition method Hydrothermal method Solvothermal method Co-precipitation method Hydrothermal method Electrodeposition method Microwave-assisted hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method Co-precipitation method Co-precipitation method Co-precipitation method Co-precipitation method solid-state reaction solid-state reaction Hydrothermal method
Na3V2(PO4)2F3 particle VS2 nanosheet MoS2 nanosheet MoS2 nanosheet MoS2 nanosheet Layered ribbon-like hydroquinone (HqTp)
sol-gel method Hydrothermal method Hydrothermal method Hydrothermal method Hydrothermal method solid-state mechano-mixing
replacing the O in C–O–C bonds with N. Nitrogen substitution can improve the poor electrochemical performance of NTCDA. In 2 M ZnSO4 aqueous electrolyte, the RZIB based on NTCDI cathode and Zn anode presents a high reversible capacity of 240 mAh g 1 at 0.1 A g-1 and capacity retention of 73.7% after 2000 cycles at 1 A g 1. The structural regulation strategy in NTCDI creates a new chance for designing cathode material for zinc storage.
140 C 140 � C 140 � C 120 � C 120 � C 200 � C 140 � C
24 h 24 h 24 h 12 h 12 h 10min 12 h
350 � C 160 � C 180 � C
5h 24 h 12 h
180 � C
180 � C 200 � C 180 � C 200 � C 200 � C 220 � C 200 � C 180 � C 180 � C
90min 72 h 48 h 48 h 48 h 48 h 48 h 60 h 24 h
180 � C
180 � C 180 � C 200 � C 190 � C
20 h 24 h 18 h 24 h
no no no no no no no no no 200 � C/24 h no no no 600 � C/4 h no 350 � C/2 h no no no no no no no 250 � C/2 h no 400 � C/3 no no no no 1000 � C/24 h 1000 � C/7 h 350 � C/5 h 750 � C/8 h 650 � C/8 h no no 250 � C/2 h no no
                                      
materials have been proposed: (1) the reversible insertion/extraction of zinc ions into/from MnO2; (2) Zn2þ was deposited on the surface of MnO2 and formed zinc hydroxide sulfate (Zn4(OH)6(SO4)⋅5H2O); and (3) reversible Zn2þ/Hþ co-insertion/extraction mechanism. Although manganese-based oxide materials have been explored widely, its reversible phase transition during charge/discharge process easily leads to an excessive structural stress, resulting in the formation of amorphous phase and decay of capacity. Vanadium-based cathode materials have also been developed because of its open-framework crystal structure, multiple oxidation states of vanadium and simple zinc ion insertion/extraction reaction mechanism. Compared with manganese-based materials, the vanadiumbased cathode materials improved effectively the cycle stability and rate performance of RZIBs because interlayer metal ions (Na, Ca, Zn, Mg, Ag, Li …) in the layered structure act as pillars to minimize the steric hin drance, but have lower voltage platform. Prussian blue analogue cath odes have large open-framework structures, their low capacity (~50 mAh g 1) and O2 evolution at high voltage (~1.7 V vs. Zn2þ/Zn) hinder their further application. Currently, the researches on Chevrel phases, polyanionic compounds and organic quinone compounds have just started and the relevant reports are few, and their capacity and rate performance need to be further improved. In brief, the development of the RZIBs is still in the primary stage, which requires increasing research efforts to achieve industrialization, especially in terms of cathode materials. In synthesis of cathode materials of RZIBs, the synthesis methods and synthesis conditions often play a crucial role in deciding the particle size, crystallinity, morphology, structure and electrochemical
9. Conclusions and future outlook Plenty of investigations show that rechargeable zinc-ion batteries (RZIBs) are one of the most promising energy storage systems to replace lithium-ion batteries. The charge storage mechanism of RZIBs is estab lished on the migration of Zn2þ ions between cathode and anode ma terials. The cathode material is the most critical component of RZIBs, determining the performance of whole RZIBs. Although cathode mate rials have progressed in recent years, there are still significant challenges to overcome before reaching large-scale commercialization. In this re view, the synthesis, composition, structure and electrochemical prop erties of various cathode materials of RZIBs have been summarize, which include manganese-based oxide, vanadium-based materials, Prussian blue analogues, Chevrel phases, polyanionic compounds, metal disulfides and organic compounds. Manganese-based dioxides have been widely used as cathode materials of RZIBs because of high elec trochemically active, environmentally friendly and relatively cheap. Manganese-oxide cathode materials include α-, β-, γ-, ε-, δ-, todorokiteMnO2 with different tunnel features and spinel ZnMn2O4. At present, three energy storage mechanism of manganese-based dioxide cathode 14
C. Li et al.
Journal of Power Sources 449 (2020) 227596
Table 5 Electrochemical performances of RZIBs based on various cathodes and electrolytes. Cathode material
Average discharge voltage(V)
MnO2: carbon black: PVDF ¼ 7:2:1
1 M ZnSO4 or Zn(NO3)2
MnO2: carbon black: PVDF ¼ 7:1:2
1 M ZnSO4
MnO2: carbon black: PVDF ¼ 7:1:2
1 M ZnSO4
MnO2: carbon black: PVDF ¼ 7:2:1
α-MnO2  α-MnO2 
MnO2: carbon black: LA133 water based adhesives: CMC ¼ 7:2:0.8:0.2 MnO2: Super-P: PTFE ¼ 7:2:1
MnO2: Super-P: CMC ¼ 8:1:1
MnO2: Ketjen black: TAB ¼ 7:2:1
2 M ZnSO4 þ 0.1 M MnSO4 2 M ZnSO4 þ 0.5 M MnSO4 2 M ZnSO4 þ 0.2 M MnSO4 1 M ZnSO4þ 0.1 M MnSO4 1 M ZnSO4
MnO2þCFP (carbon fiber paper)
MnO2: Ketjen black: TAB ¼ 7:2:1
2 M ZnSO4 þ 0.2 M MnSO4 1 M ZnSO4
0.5 M Zn(TFSI)2 in acetonitrile
210 mAh g 1 at 0.5C 194 mAh g 1 at C/ 20 167 mAh g 1 at C/ 5 285 mAh g 1 at C/ 3 665 mAh g 1 at 100 mA g 1 382 mAh g 1 at 300 mA g 1 270 mAh g 1 at 100 mA g 1 285 mAh g 1 at 0.05 mA cm 2 260 mAh g 1 at 1.3C 250 mAh g 1 at 83 mA g 1 123 mAh g 1 at 12.3 mA g 1
100% retained after 100 cycles at 6C 65% retained after 30 cycles at C/20 70% retained after 30 cycles at C/5 92% retained after 5000 cycles at 5C 99% retained after 500 cycles at 5000 mA g 1 94% retained after 3000 cycles at 3000 mA g 1 75% retained after 200 cycles at 200 mA g 1 63% retained after 40 cycles at 0.5 mA cm 2 99% retained after 10000 cycles at 6.5 C 46% retained after 100 cycles at 83 mA g 1 48% retained after 125 cycles at 12.3 mA g 1
Todorokite MnO2 
MnO2: carbon black: PVDF ¼ 8.5:1:0.5
1 M ZnSO4
Spinel ZnMn2O4 
ZnMn2O4: PVDF ¼ 9:1
3 M Zn(CF3SO3)2
Spinel ZnMn2O4 
MnO2: acetylene black: PVDF ¼ 8:1:1
1 M ZnSO4 þ 0.05 M MnSO4 3 M ZnSO4
V2O5: acetylene black: PVDF ¼ 7:2:1
V2O5: Super-P: PVDF ¼ 7:2:1
1 M Zn(CF3SO3)2 þ 21 M LiTFSI 0.5 M Zn(TFSI)2 in acetonitrile 3 M Zn(CF3SO3)2
Zn0.25V2O5: Super-P: CMC:SBR ¼ 7:2.7:0.2:0.1 Ca0.25V2O5: Super-P: CMC:SBR ¼ 7:2.7:0.2:0.1 Na0.33V2O5: Super-P: PVDF ¼ 7:2:1
1 M ZnSO4
1 M ZnSO4
108 mAh g 1 at C/ 2 150 mAh g 1 at 50 mA g 1 70.2 mAh g 1 at 3000 mA g 1 224 mAh g 1 at 100 mA g 1 238 mAh g 1 at 50 mA g 1 196 mAh g 1 at C/ 10 381 mAh g 1 at 60 mA g 1 282 mAh g 1 at 300 mA g 1 289 mAh g 1 at 1C
3 M Zn(CF3SO3)2
1.10&0.79, 0.63& 0.52
367.1 mAh g 100 mA g 1
83% retained after 50 cycles at C/2 94% retained after 500 cycles at 500 mA g 1 106.5 mAh g 1 after 300 cycles at 100 mA g 1 44% retained after 100 cycles at 500 mA g 1 80% retained after 2000 cycles at 2000 mA g 1 87% retained after 120 cycles at C/10 71% retained after 900 cycles at 6000 mA g 1 81% retained after 1000 cycles at 2400 mA g 1 96% retained after 3000 cycles at 80C 93% retained after 1000 cycles at 200 mA g 1
3 M Zn(CF3SO3)2
Ca0.25V2O5⋅nH2O  Na0.33V2O5  MgxV2O5⋅nH2O 
1.60&1.38 1.25&1.38 1.60&1.25 1.30&1.20
MgxV2O5: single wall carbon nanotubes: CMC: SBR ¼ 7:2.7:0.2:0.1 353 mAh g 1 at 50 mA g 1
LixV2O5: acetylene black: PVDF ¼ 7:2:1
97% retained after 2000 cycles at 5000 mA g 1 2 M ZnSO4
H2V3O8: acetylene black: PVDF ¼ 7:2:1
3 M Zn(CF3SO3)2
Na2V6O16: acetylene black: PVDF ¼ 7:2:1
3 M Zn(CF3SO3)2
ZnHCF: Super-P: PVDF: KS6 ¼ 7.5:1.2:1:0.3 CuHCF: Super-P: PVDF: SFG6 ¼ 8:0.9:0.9:0.2 K0.86Ni[Fe(CN)6]0.954(H2O)0.766: SuperP: PVDF ¼ 7:2:1
1 M ZnSO4
0.02 M ZnSO4
0.5 M Zn(ClO4)2 in acetonitrile
1 M Zn(OAc)2 in [Ch] OAc þ water 1 M ZnSO4
FeFe(CN)6: amorphous carbon: PVDF: SFG6 ¼ 8:1:0.8:0.2 Mo6S8: Super-P: PVDF ¼ 8:1:1
Mo6S8: Super-C: PVDF ¼ 8:1:1
1 M ZnSO4
0.5 M Zn(CH3COO)2
Na3V2(PO4)3: acetylene black: PVDF ¼ 8:2:1 Na3V2(PO4)2F3: Super-P: PTFE ¼ 7:2:1
2 M Zn(CH3F3SO3)2
Quinone (C4Q) 
C4Q: Super-P: PVDF ¼ 6:3.5:0.5
3 M Zn(CH3F3SO3)2
p-chloranil: Super-P: CMC/SBR(2:1) ¼ 6:3.5:0.5
1 M Zn(OTf)2-H2O
CuHCF  K0.86Ni[Fe (CN)6]0.954(H2O)0.766  FeFe(CN)6 
407.6 mAh g 1 at 1000 mA g 1 423.8 mAh g 1 at 100 mA g 1 352 mAh g 1 at 50 mA g 1 60.4 mAh g 1 at 120 mA g 1 53 mAh g 1 at 60 mA g 1 26.8 mAh g 1 at 56 mA g 1
76% retained after 500 cycles at 5000 mA g 1 94% retained after 1000 cycles at 5000 mA g 1 90% retained after 6000 cycles at 5000 mA g 1 76% retained after 100 cycles at 300 mA g 1 96% retained after 100 cycles at 60 mA g 1 96% retained after 35 cycles at 56 mA g 1
120 mAh g 1 at 10 mA g 1 134 mAh g 1 at 6.4 mA g 1 63 mAh g 1 at 180 mA g 1
95% retained after 10 cycles at 10 mA g 1 /
97 mAh g 1 at 0.5C 60 mAh g 1 at 200 mA g 1 335 mAh g 1 at 20 mA g 1 200 mAh g 1 at 217 mA g 1
74% retained after 100 cycles at 0.5C 95% retained after 4000 cycles at 1000 mA g 1 87% retained after 1000 cycles at 500 mA g 1 53% retained after 100 cycles at 43.4 mA g 1
95% retained after 150 cycles at 180 mA g 1
C. Li et al.
Journal of Power Sources 449 (2020) 227596
performances of cathode materials. We have summarized the synthesis methods and synthesis conditions of various cathode materials with different structures for RZIBs (Table 4), including microemulsion method, hydrothermal method, microwave-assisted hydrothermal method, electrodeposition method, thermal decomposition method and co-precipitation method, etc. Each synthesis method has unique ad vantages and functional features as well as disadvantages. Among various synthetic methods, the hydrothermal method not only is an easy route for obtaining cathode materials with high particle purity, good dispersity, good and controllable crystal shape, but also has low syn thesis cost and low synthesis temperature. However, this method needs high technology and high equipment requirements, and has poor safety performance and long preparation period. So it is difficult to achieve mass production of cathode materials for RZIBs. Microwave-assisted hydrothermal method can effectively shorten the reaction time within a few hours and accelerate the reaction process of synthesis. Most liquid methods, such as microemulsion method, electrodeposition method and co-precipitation method, etc. do not require high processing tempera tures, expensive and complicated laboratory equipment, but have low particle purity, poor dispersity and crystal shape as well as sinterability. The results show that the type (e.g. nanorod or nanowire) of final cathode material for RZIBs determined the choice of synthesis methods. Although the synthesis technologies of cathode materials for RZIBs have been developed rapidly in recent years, there is a great need to develop new methods for synthesizing nanostructured electrodes with large inter-layer spacing. Table 5 is the electrochemical performances of RZIBs based on various cathodes and electrolytes. According to this overview, further research directions and per spectives regarding the development of high performance RZIBs are proposed as follows: (1) The larger electrostatic interaction of the Zn cation with its surrounding electrolyte and electrode materials leads to extremely slow intercalation kinetics. A good method to solve this problem is synthesizing nano-sized materials. Nano-sized electrodes intrinsically benefit rapid ionic diffusion due to short transport distance and better accommodate the structural strain through slippage at domain boundaries. (2) Tailoring crystal orientation for electrode ma terials is also an attractive strategy because the exposure of specific planes of crystal structure promotes ionic transports on its exposure surface, further demonstrating high discharge capacity as well as high rate capability [168,169]. (3) It’s worth noting that cation-defective materials by using cation nonstoichiometry can open up additional pathways for easier migration of multivalent metal-ions, which endue us another chance to acquire advanced electrode materials. (4) The emergence of flexible and wearable RZIBs provides a new opportunity for the application in wearable devices. Under this circumstance, RZIBs need to sustain harsher conditions such as folding, hitting puncture, tearing or immersion in water while exhibit a superior performance [170,171]. For example, Li et al.  fabricated an extremely safe, wearable and solid-state RZIB using novel gelatin and polyacrylamide (PAM) based hierarchical polymer electrolyte (HPE) and α-MnO2 nanorod/carbon nanotube (CNT) cathode. This RZIB delivers superior specific capacity of 306 mAh g 1 and 97% capacity retention after 1000 cycles under various severe conditions, which is able to power a com mercial smart watch and a wearable pulse sensor. Li et al.  pre pared MoS2 (E-MoS2) cathode with the expanded inter-layer spacing by an electrodeposition approach and constructed a flexible solid-state RZIB based on this cathode, new Starch/PAM hydrogel electrolyte, and Zn anode. The Starch/PAM hydrogel electrolyte with a 3D porous architecture contributes to a high water-retention capability and fast ion diffusion. This battery shows a specific discharge capacity of 199.3 mAh g 1 at 100 mA g 1 and capacity retention is 97.7% over 500 cycles at 1000 mAg 1. Furthermore, it also has high flexibility, mechanical robustness and electrochemical stability under various deformation conditions. Zhang et al.  designed a coaxial-fiber aqueous RZIB by adopting Zn nanosheet arrays on carbon nanotube fiber as the core electrode and spherical zinc hexacyanoferrate (ZnHCF) composite on
aligned carbon nanotube sheets as the outer electrode with ZnSO4- carboxymethyl cellulose sodium gel electrolyte. This RZIB delivers excellent flexibility with the capacity retention of 93.2% after bending 3000 times. Wang et al.  fabricated a novel wire-shaped flexible RZIB based on Nitinol shape memory wire, stainless steel yarn and gelatin-borax complex electrolyte. Zinc anode and MnO2 cathode are electrodeposited onto Nitinol wire and stainless steel yarn, respectively. Impressively, this flexible wire-shaped battery could recover both the shape and the electrochemical performances for multiple times once being heavily bended with permanent strain due to the shape memory effect provided by the Nitinol wire, showing excellent durability and stability. All in all, we hope this review offers motivation and inspiration for researchers to discover novel cathode materials and narrow the gap for commercialization of low cost, safe and high energy density RZIBs. Declaration of competing interest The authors declare that they have no known competing financial interests or personal relationships that could have appeared to influence the work reported in this paper. Acknowledgements This work was supported by the Nation Natural Science Foundation of China (grant numbers 51672139, 51472127 and 51272144). References  Y. Wang, B. Liu, Q. Li, S. Cartmell, S. Ferrara, J. Power Sources 286 (2015) 330–345.  G. Zubi, R. Dufo-L� opez, M. Carvalho, G. Pasaoglu, Renew. Sustain. Energy Rev. 89 (2018) 292–308.  N. Nitta, F. Wu, J.T. Lee, G. Yushin, Mater. Today 18 (2015) 252–264.  G. Liang, X. Qin, J. Zou, L. Luo, Y. Wang, M. Wu, H. Zhu, G. Chen, F. Kang, B. Li, Carbon 127 (2018) 424–431.  B. Luo, Y. Hu, X. Zhu, T. Qiu, L. Zhi, M. Xiao, H. Zhang, M. Zou, A. Cao, L. Wang, J. Mater. Chem. 6 (2018) 1462–1472.  Y.J. Nam, D.Y. Oh, S.H. Jung, Y.S. Jung, J. Power Sources 375 (2018) 93–101.  X. Tao, Y. Liu, W. Liu, G. Zhou, J. Zhao, D. Lin, C. Zu, O. Sheng, W. Zhang, H. W. Lee, Y. Cui, Nano Lett. 17 (2017) 2967–2972.  A. Eftekhari, D.W. Kim, J. Power Sources 395 (2018) 336–348.  J.S. Park, J. Kim, J.H. Jo, S.T. Myung, J. Mater. Chem. 6 (2018) 16627–16637.  T. Liu, Y. Zhang, Z. Jiang, X. Zeng, J. Ji, Z. Li, X. Gao, M. Sun, Z. Lin, M. Ling, J. Zheng, C. Liang, Energy Environ. Sci. 12 (2019) 1512–1533.  X. Hu, X. Sun, S.J. Yoo, B. Evanko, F. Fan, S. Cai, C. Zheng, W. Hu, G.D. Stucky, Nano Energy 56 (2019) 828–839.  Y. Lee, J.K. Yoo, Y. Oh, H. Park, W. Go, S.T. Myung, J. Kim, J. Mater. Chem. 6 (2018) 17571–17578.  M. Song, H. Tan, D. Chao, H.J. Fan, Adv. Funct. Mater. 28 (2018) 1802564.  D. Selvakumaran, A. Pan, S. Liang, J. Mater. Chem. 7 (2019) 18209–18236.  J. Ming, J. Guo, C. Xia, W. Wang, H.N. Alshareef, Mater. Sci. Eng. R 135 (2019) 58–84.  V. Verma, S. Kumar, W. Manalastas Jr., R. Satish, M. Srinivasan, Adv. Sustain. Syst. 3 (2019) 1800111.  M.M. Huie, D.C. Bock, E.S. Takeuchi, A.C. Marschilok, K.J. Takeuchi, Coord. Chem. Rev. 287 (2015) 15–27.  X. Deng, Y. Xu, Q. An, F. Xiong, S. Tan, L. Wu, L. Mai, J. Mater. Chem. 7 (2019) 10644–10650.  R.J. Gummow, G. Vamvounis, M.B. Kannan, Y. He, Adv. Mater. 30 (2018) 1801702.  P. Padigi, G. Goncher, D. Evans, R. Solanki, J. Power Sources 273 (2015) 460–464.  Q. Li, N.J. Bjerrum, J. Power Sources 110 (2002) 1–10.  T. Cai, L. Zhao, H. Hu, T. Li, X. Li, S. Guo, Y. Li, Q. Xue, W. Xing, Z. Yan, L. Wang, Energy Environ. Sci. 11 (2018) 2341–2347.  W. Liu, J. Hao, C. Xu, J. Mou, L. Dong, F. Jiang, Z. Kang, J. Wu, B. Jiang, F. Kang, Chem. Commun. 53 (2017) 6872–6874.  H.B. Zhao, C.J. Hu, H.W. Cheng, J.H. Fang, Y.P. Xie, W.Y. Fang, T.N.L. Doan, T.K. A. Hoang, J.Q. Xu, P. Chen, Sci. Rep. 6 (2016) 25809.  L. Chen, Q. An, L. Mai, Adv. Mater. Interfaces 6 (2019) 1900387.  D.R. Gabe, J. Appl. Electrochem. 27 (1997) 908–915.  X. Wang, F. Wang, L. Wang, M. Li, Y. Wang, B. Chen, Y. Zhu, L. Fu, L. Zha, L. Zhang, Y. Wu, W. Huang, Adv. Mater. 28 (2016) 4904–4911.  J.F. Parker, C.N. Chervin, I.R. Pala, M. Machler, M.F. Burz, J.W. Long, D. R. Rolison, Science 356 (2017) 415–418.  H. Li, C. Xu, C. Han, Y. Chen, C. Wei, B. Li, F. Kang, J. Electrochem. Soc. 162 (2015) A1439–A1444.
C. Li et al.                                             
       
Journal of Power Sources 449 (2020) 227596
W. Li, K. Wang, S. Cheng, K. Jiang, Energy Storage Mater. 15 (2018) 14–21. G. Fang, J. Zhou, A. Pan, S. Liang, ACS Energy Lett. 3 (2018) 2480–2501. Z. Liu, P. Bertram, F. Endres, J. Solid State Electrochem. 21 (2017) 2021. M. Petkovic, K.R. Seddon, L.P.N. Rebelo, C.S. Pereira, Chem. Soc. Rev. 40 (2011) 1383–1403. R.K. Guduru, J.C. Icaza, Nanomaterials 6 (2016) 41. L. Zhang, L. Chen, X. Zhou, Z. Liu, Sci. Rep. 5 (2015) 18263. W. Liang, L. Wang, H. Zhu, Y. Pan, Z. Zhu, H. Sun, C. Ma, A. Li, Sol. Energy Mater. Sol. Cells 180 (2018) 158–167. M. Cakici, R.R. Kakarla, F. Alonso-Marroquin, Chem. Eng. J. 309 (2017) 151–158. C.J. Raj, K.B.R. Varma, Electrochim. Acta 56 (2010) 649–656. P.K. Gupta, A. Bhandari, J. Bhattacharya, R.G.S. Pala, J. Phys. Chem. C 12 (2018) 211689–211700. S. Zhu, L. Li, J. Liu, H. Wang, T. Wang, Y. Zhang, L. Zhang, R.S. Ruoff, F. Dong, ACS Nano 12 (2018) 1033–1042. S. Devaraj, N. Munichandraiah, J. Phys. Chem. C 112 (2008) 4406–4417. C. Xu, B. Li, H. Du, F. Kang, Angew. Chem., Int. Ed. Engl. 51 (2012) 933–935. F.Y. Cheng, J. Chen, L. Gou, P.W. Shen, Adv. Mater. 17 (2005) 2753. C. Xu, S.W. Chiang, J. Ma, F. Kang, J. Electrochem. Soc. 160 (2013) A93–A97. L. Athouel, F. Moser, R. Dugas, O. Crosnier, D. Belanger, T. Brousse, J. Phys. Chem. C 112 (2008) 7270–7277. A.S. Poyraz, J. Huang, S. Cheng, L. Wu, X. Tong, Y. Zhu, A.C. Marschilok, K. J. Takeuchi, E.S. Takeuchi, J. Electrochem. Soc. 164 (2017) A1983–A1990. C. Xu, C. Wei, B. Li, F. Kang, Z. Guan, J. Power Sources 196 (2011) 7854–7859. B. Lee, C.S. Yoon, H.R. Lee, K.Y. Chung, B.W. Cho, S.H. Oh, Sci. Rep. 4 (2014) 6066. A.D. Wadsley, Nature 172 (1953) 1103–1104. A.D. Wadsley, Acta Crystallogr. 8 (1955) 165–172. B. Lee, H.R. Lee, H. Kim, K.Y. Chung, B.W. Cho, S.H. Oh, Chem. Commun. 51 (2015) 9265–9268. J.E. Post, Proc. Natl. Acad. Sci. U.S.A. 96 (1999) 3447–3454. W. Wang, B. Jiang, W. Xiong, H. Sun, Z. Lin, L. Hu, J. Tu, H. Zhu, S. Jiao, Sci. Rep. 3 (2013) 3383. M. Villalobos, B. Lanson, A. Manceau, B. Toner, G. Sposito, Am. Mineral. 91 (2006) 489–502. K.D. Kwon, K. Refson, G. Sposito, Geochem. Cosmochim. Acta 73 (2009) 1273–1284. B. Lee, H.R. Seo, H.R. Lee, C.S. Yoon, J.H. Kim, K.Y. Chung, B.W. Cho, S.H. Oh, ChemSusChem 9 (2016) 1–10. T. Takashima, K. Hashimoto, R. Nakamura, J. Am. Chem. Soc. 134 (2012) 18153–18156. W.K. Pang, V.K. Peterson, N. Sharma, C.F. Zhang, Z.P. Guo, J. Phys. Chem. C 118 (2014) 3976–3983. J.E. Greedan, N.P. Raju, A.S. Wills, C. Morin, S.M. Shaw, J.N. Reimers, Chem. Mater. 10 (1998) 3058–3067. J.C. Hunter, J. Solid State Chem. 39 (1981) 142–147. A. Moezzi, M.B. Cortie, A.M. McDonagh, Dalton Trans. 42 (2013) 14432–14437. H. Pan, Y. Shao, P. Yan, Y. Cheng, K.S. Han, Z. Nie, C. Wang, J. Yang, X. Li, P. Bhattacharya1, K.T. Mueller, J. Liu, Nat. Energy 1 (2016) 16039. F. Jiao, P.G. Bruce, Adv. Mater. 19 (2007) 657–660. D. Su, H.-J. Ahn, G. Wang, J. Mater. Chem. 1 (2013) 4845–4850. S. Islam, M.H. Alfaruqi, V. Mathew, J. Song, S. Kim, S. Kim, J. Jo, J.P. Baboo, D. T. Pham, D.Y. Putro, Y.K. Sun, J. Kim, J. Mater. Chem. 5 (2017) 23299–23309. N. Zhang, F. Cheng, J. Liu, L. Wang, X. Long, X. Liu, F. Li, J. Chen, Nat. Commun. 8 (2017) 405. J.H. Zeng, Y.F. Wang, Y. Yang, J. Zhang, J. Mater. Chem. 20 (2010) 10915–10918. V. Mathew, J. Lim, J. Kang, J. Gim, A.K. Rai, J. Kim, Electrochem. Commun. 13 (2011) 730–733. E. Chae, J. Gim, J. Song, S. Kim, V. Mathew, J. Han, S. Boo, J. Kim, RSC Adv. 3 (2013) 26328–26333. M.H. Alfaruqi, V. Mathew, J. Gim, S. Kim, J. Song, J.P. Baboo, S.H. Choi, J. Kim, Chem. Mater. 27 (2015) 3609–3620. W.I.F. David, M.M. Thackeray, P.G. Bruce, J.B. Goodenough, Mater. Res. Bull. 19 (1984) 99–106. W. Sun, F. Wang, S. Hou, C. Yang, X. Fan, Z. Ma, T. Gao, F. Han, R. Hu, M. Zhu, C. Wang, J. Am. Chem. Soc. 139 (2017) 9775–9778. M.H. Alfaruqi, J. Gim, S. Kim, J. Song, D.T. Pham, J. Jo, Z. Xiu, V. Mathew, J. Kim, Electrochem. Commun. 60 (2015) 121–125. S.D. Han, S. Kim, D. Li, V. Petkov, H.D. Yoo, P.J. Phillips, H. Wang, J.J. Kim, K. L. More, B. Key, R.F. Klie, J. Cabana, V.R. Stamenkovic, T.T. Fister, N. M. Markovic, A.K. Burrell, S. Tepavcevic, J.T. Vaughey, Chem. Mater. 29 (2017) 4874–4884. J. Muldoon, C.B. Bucur, T. Gregory, Chem. Rev. 114 (2014) 11683–11720. H.D. Yoo, I. Shterenberg, Y. Gofer, G. Gershinsky, N. Poura, D. Aurbach, Energy Environ. Sci. 6 (2013) 2265–2279. S.-D. Han, N.N. Rajput, X. Qu, B. Pan, M. He, M.S. Ferrandon, C. Liao, K. A. Persson, ACS Appl. Mater. Interfaces 8 (2016) 3021–3031. C. Yuan, Y. Zhang, Y. Pan, X. Liu, G. Wang, D. Cao, Electrochim. Acta 116 (2014) 404–412. C. Wei, C. Xu, B. Li, H. Du, F. Kang, J. Phys. Chem. Solids 73 (2012) 1487–1491. J. Lee, J.B. Ju, W.I. Cho, B.W. Cho, S.H. Oh, Electrochim. Acta 112 (2013) 138–143. Q. Gao, Z. Yuan, L. Dong, G. Wang, X. Yu, Electrochim. Acta 270 (2018) 417–425. M. Zhong, D. Yang, C. Xie, Z. Zhang, Z. Zhou, X.H. Bu, Small 12 (2016) 5564–5571.
 J.C. Knight, S. Therese, A. Manthiram, J. Mater. Chem. 3 (2015) 21077–21082.  T. Koketsu, J. Ma, B.J. Morgan, M. Body, C. Legein, W. Dachraoui, M. Giannini, A. Demorti� ere, M. Salanne, F. Dardoize, H. Groult, O.J. Borkiewicz, K. W. Chapman, P. Strasser, D. Dambournet, Nat. Mater. 16 (2017) 1142–1448.  L. S� anchez, J.P. Pereira-Ramos, J. Mater. Chem. 7 (1997) 471–473.  N. Zhang, F. Cheng, Y. Liu, Q. Zhao, K. Lei, C. Chen, X. Liu, J. Chen, J. Am. Chem. Soc. 138 (2016) 12894–12901.  C. Li, X. Han, F. Cheng, Y. Hu, C. Chen, J. Chen, Nat. Commun. 6 (2015) 7345.  L. Suo, O. Borodin, T. Gao, M. Olguin, J. Ho, X. Fan, C. Luo, C. Wang, K. Xu, Science 350 (2015) 938–943.  Y. Yamada, K. Furukawa, K. Sodeyama, K. Kikuchi, M. Yaegashi, Y. Tateyama, A. Yamada, J. Am. Chem. Soc. 136 (2014) 5039–5046.  X. Wu, Y. Xiang, Q. Peng, X. Wu, Y. Li, F. Tang, R. Song, Z. Liu, Z. He, X. Wu, J. Mater. Chem. 5 (2017) 17990–17997.  S. Islam, M.H. Alfaruqi, J. Song, S. Kim, D.T. Pham, J. Jo, S. Kim, V. Mathew, J. P. Baboo, Z. Xiu, J. Kim, J. Energy Chem. 26 (2017) 815–819.  B. Wu, G. Zhang, M. Yan, T. Xiong, P. He, L. He, X. Xu, L. Mai, Small 14 (2018) 1703850.  G.G. Yadav, J.W. Gallaway, D.E. Turney, M. Nyce, J. Huang, X. Wei, S. Banerjee, Nat. Commun. 8 (2017) 14424.  D. Xu, B. Li, C. Wei, Y.B. He, H. Du, X. Chu, X. Qin, Q.H. Yang, F. Kang, Electrochim. Acta 133 (2014) 254–261.  D. Imamura, Solid State Ion. 161 (2003) 173–180.  S. Gu, H. Wang, C. Wu, Y. Bai, H. Li, F. Wu, Energy Storage Mater. 6 (2017) 9–17.  J. Zhou, L. Shan, Z. Wu, X. Guo, G. Fang, S. Liang, Chem. Commun. 54 (2018) 4457–4460.  P. Hu, M. Yan, T. Zhu, X. Wang, X. Wei, J. Li, L. Zhou, Z. Li, L. Chen, L. Mai, ACS Appl. Mater. Interfaces 9 (2017) 42717–42722.  L. Suo, O. Borodin, W. Sun, X. Fan, C. Yang, F. Wang, T. Gao, Z. Ma, M. Schroeder, A. Gresce, S. Russell, M. Armand, A. Angell, K. Xu, C. Wang, Angew. Chem. Int. Ed. 55 (2016) 7136–7141.  A. Gambou-Bosca, D. B�elanger, J. Power Sources 326 (2016) 595–603.  Y. Zhao, C. Han, J. Yang, J. Su, X. Xu, S. Li, L. Xu, R. Fang, H. Jiang, X. Zou, B. Song, L. Mai, Q. Zhang, Nano Lett. 15 (2015) 2180–2185.  P. Senguttuvan, S.D. Han, S. Kim, A.L. Lipson, S. Tepavcevic, T.T. Fister, I. D. Bloom, A.K. Burrell, C.S. Johnson, Adv. Energy Mater. 6 (2016) 1600826.  S. Tepavcevic, Y. Liu, D. Zhou, B. Lai, J. Maser, X. Zuo, H. Chan, P. Kr� al, C. S. Johnson, V. Stamenkovic, N.M. Markovic, T. Rajh, ACS Nano 9 (2015) 8194–8205.  H.Y. Li, C.H. Yang, C.M. Tseng, S.W. Lee, C.C. Yang, T.Y. Wu, J.K. Chang, J. Power Sources 285 (2015) 418–424.  M. Yan, P. He, Y. Chen, S. Wang, Q. Wei, K. Zhao, X. Xu, Q. An, Y. Shuang, Y. Shao, K.T. Mueller, L. Mai, J. Liu, J. Yang, Adv. Mater. 30 (2017) 1703725.  K.W. Nam, H. Kim, J.H. Choi, J.W. Choi, Energy Environ. Sci. 12 (2019) 1999–2009.  D. Kundu, B.D. Adams, V. Duffort, S.H. Vajargah, L.F. Nazar, Nat. Energy 1 (2016) 16119.  C. Xia, J. Guo, P. Li, X. Zhang, H.N. Alshareef, Angew. Chem. Int. Ed. 57 (2018) 3943–3948.  P. He, G. Zhang, X. Liao, M. Yan, X. Xu, Q. An, J. Liu, L. Mai, Adv. Energy Mater. 8 (2018) 1702463.  L. Shan, Y. Yang, W. Zhang, H. Chen, G. Fang, J. Zhou, S. Liang, Energy Storage Mater. 18 (2019) 10–14.  V. Bodenez, L. Dupont, M. Morcrette, C. Surcin, D.W. Murphy, J.M. Tarascon, Chem. Mater. 18 (2006) 4278–4287.  K. Kirshenbaum, D.C. Bock, C.Y. Lee, Z. Zhong, K.J. Takeuchi, A.C. Marschilok, E. S. Takeuchi, Science 347 (2015) 149–154.  E.S. Takeuchi, A.C. Marschilok, K.J. Takeuchi, A. Ignatov, Z. Zhong, M. Croft, Energy Environ. Sci. 6 (2013) 1465–1470.  L. Shan, J. Zhou, M. Han, G. Fang, X. Cao, X. Wu, S. Liang, J. Mater. Chem. 7 (2019) 7355–7359.  F. Ming, H. Liang, Y. Lei, S. Kandambeth, M. Eddaoudi, H.N. Alshareef, ACS Energy Lett. 3 (2018) 2602–2609.  Y. Yang, Y. Tang, G. Fang, L. Shan, J. Guo, W. Zhang, J. Zhou, C. Wang, L. Wang, S. Liang, Energy Environ. Sci. 11 (2018) 3157–3162.  C. Xia, J. Guo, Y. Lei, H. Liang, C. Zhao, H.N. Alshareef, Adv. Mater. 30 (2018) 1705580.  W. Kaveevivitchai, A. Manthiram, J. Mater. Chem. 4 (2016) 18737–18741.  J.H. Jo, Y.K. Sun, S.T. Myung, J. Mater. Chem. 5 (2017) 8367–8375.  M.H. Alfaruqi, V. Mathew, J. Song, S. Kim, J.P. Baboo, Z. Xiu, K.S. Lee, Y.K. Sun, J. Kim, Chem. Mater. 29 (2017) 1684–1694.  P. He, Y. Quan, X. Xu, M. Yan, W. Yang, Q. An, L. He, L. Mai, Small 13 (2017) 1702551.  P. Hu, T. Zhu, X. Wang, X. Wei, M. Yan, J. Li, W. Luo, W. Yang, W. Zhang, L. Zhou, Z. Zhou, L. Mai, Nano Lett. 18 (2018) 1758–1763.  F. Wan, L. Zhang, X. Dai, X. Wang, Z. Niu, J. Chen, Nat. Commun. 9 (2018) 1656.  B. Tang, G. Fang, J. Zhou, L. Wang, Y. Lei, C. Wang, T. Lin, Y. Tang, S. Liang, Nano Energy 51 (2018) 579–587.  X. Guo, G. Fang, W. Zhang, J. Zhou, L. Shan, L. Wang, C. Wang, T. Lin, Y. Tang, S. Liang, Adv. Energy Mater. 8 (2018) 1801819.  H. Li, T. Zhai, P. He, Y. Wang, E. Hosono, H. Zhou, J. Mater. Chem. 21 (2011) 1780–1787.  G. Fang, S. Liang, Z. Chen, P. Cui, X. Zheng, A. Pan, B. Lu, X. Lu, J. Zhou, Adv. Funct. Mater. 29 (2019) 1905267.  A. Kumar, S.M. Yusuf, L. Keller, Phys. Rev. B 71 (2005), 054414.
C. Li et al.
Journal of Power Sources 449 (2020) 227596  C. Zhao, C. Yu, M. Zhang, Q. Sun, S. Li, M.N. Banis, X. Han, Q. Dong, J. Yang, G. Wang, X. Sun, J. Qiu, Nano Energy 41 (2017) 66–74.  P. He, M. Yan, G. Zhang, R. Sun, L. Chen, Q. An, L. Mai, Adv. Energy Mater. 7 (2017) 1601920.  H. Liang, Z. Cao, F. Ming, W. Zhang, D.H. Anjum, Y. Cui, L. Cavallo, H. N. Alshareef, Nano Lett. 19 (2019) 3199–3206.  W. Xu, C. Sun, K. Zhao, X. Cheng, S. Rawal, Y. Xu, Y. Wang, Energy Storage Mater. 16 (2019) 527–534.  K. Lin, Q. Chen, M.R. Gerhardt, L. Tong, S.B. Kim, L. Eisenach, A.W. Valle, D. Hardee, R.G. Gordon, M.J. Aziz, M.P. Marshak, Science 349 (2015) 1529–1532.  T.B. Schon, B.T. McAllister, P.-F. Li, D.S. Seferos, Chem. Soc. Rev. 45 (2016) 6345–6404.  Y. Liang, Y. Jing, S. Gheytani, K.-Y. Lee, P. Liu, A. Facchetti, Y. Yao, Nat. Mater. 16 (2017) 841–848.  X. Dong, L. Chen, J. Liu, S. Haller, Y. Wang, Y. Xia, Sci. Adv. 2 (2016), e1501038.  Q. Zhao, W. Huang, Z. Luo, L. Liu, Y. Lu, Y. Li, L. Li, J. Hu, H. Ma, J. Chen, Sci. Adv. 4 (2018) 2375–2548.  B.S. Creaven, D.F. Donlon, J. McGinley, Coord. Chem. Rev. 253 (2009) 893–962.  D. Kundu, P. Oberholzer, C. Glaros, A. Bouzid, E. Tervoort, A. Pasquarello, M. Niederberger, Chem. Mater. 30 (2018) 3874–3881.  A. Khayum, M. Ghosh, V. Vijayakumar, A. Halder, M. Nurhuda, S. Kumar, M. Addicoat, S. Kurungot, R. Banerjee, Chem. Sci. 10 (2019) 8889–8894.  X. Wang, L. Chen, F. Lu, J. Liu, X. Chen, G. Shao, ChemElectroChem 6 (2019) 3644–3647.  F. Wang, X. Wang, Z. Chang, Y. Zhu, L. Fu, X. Liu, Y. Wu, Y. Wu, W. Huang, A. Subramanian, H. Fan, L. Qi, A. Kushima, J. Li, Y. Lin, K. Xu, L.W. Wang, Y. P. Wu, F. Pan, Nanoscale Horiz. 1 (2016) 272–289.  L. Wang, X. He, W. Sun, J. Wang, Y. Li, S. Fan, Nano Lett. 12 (2012) 5632–5636.  A. Konarov, N. Voronina, J.H. Jo, Z. Bakenov, Y.K. Sun, S.T. Myung, ACS Energy Lett. 3 (2018) 2620–2640.  P.H. Yang, K. Liu, Q. Chen, X.B. Mo, Y.S. Zhou, S. Li, G. Feng, J. Zhou, Angew. Chem. Int. Ed. 55 (2016) 12050–12053.  H. Li, C. Han, Y. Huang, Y. Huang, M. Zhu, Z. Pei, Q. Xue, Z. Wang, Z. Liu, Z. Tang, Y. Wang, F. Kang, B. Li, C. Zhi, Energy Environ. Sci. 11 (2018) 941–951.  H. Li, Q. Yang, F. Mo, G. Liang, Z. Liu, Z. Tang, L. Ma, J. Liu, Z. Shi, C. Zhi, Energy Storage Mater. 19 (2019) 94–101.  Q. Zhang, C. Li, Q. Li, Z. Pan, J. Sun, Z. Zhou, B. He, P. Man, L. Xie, L. Kang, X. Wang, J. Yang, T. Zhang, P.P. Shum, Q. Li, Y. Yao, L. Wei, Nano Lett. 19 (2019) 4035–4042.  Z. Wang, Z. Ruan, Z. Liu, Y. Wang, Z. Tang, H. Li, M. Zhu, T.F. Hung, J. Liu, Z. Shi, C. Zhi, J. Mater. Chem. 6 (2018) 8549–8557.
 P. Padigi, J. Thiebes, M. Swan, G. Goncher, D. Evans, Electrochim. Acta 166 (2015) 32–39.  H. Lee, Y.I. Kim, J.K. Park, J.W. Choi, Chem. Commun. 48 (2012) 8416–8418.  P. Nie, L. Shen, H. Luo, B. Ding, G. Xu, J. Wang, X. Zhang, J. Mater. Chem. 2 (2014) 5852–5857.  S. Liu, G.L. Pan, G.R. Li, X.P. Gao, J. Mater. Chem. 3 (2015) 959–962.  R.Y. Wang, C.D. Wessells, R.A. Huggins, Y. Cui, Nano Lett. 13 (2013) 5748–5752.  L. Zhang, L. Chen, X. Zhou, Z. Liu, Adv. Energy Mater. 5 (2014) 1400930.  J.J. Alexander, H.B. Gray, J. Am. Chem. Soc. 90 (1968) 4260–4271.  R. Tr� ocoli, F.L. Mantia, ChemSusChem 8 (2015) 481–485.  M.S. Chae, J.W. Heo, H.H. Kwak, H. Lee, S.T. Hong, J. Power Sources 337 (2017) 204–211.  Z. Liu, G. Pulletikurthi, F. Endres, ACS Appl. Mater. Interfaces 8 (2016) 12158–12164.  M. Pasta, C.D. Wessells, N. Liu, J. Nelson, M.T. McDowell, R.A. Huggins, M. F. Toney, Y. Cui, Nat. Commun. 5 (2014) 3007.  E. Levi, G. Gershinsky, D. Aurbach, O. Isnard, G. Ceder, Chem. Mater. 21 (2009) 1390–1399.  S. Belin, R. Chevrel, M. Sergent, J. Solid State Chem. 155 (2000) 250–258.  J.H. Cho, J.H. Ha, J.G. Lee, C.S. Kim, B.W. Cho, K.B. Kim, K.Y. Chung, J. Phys. Chem. C 121 (2017) 12617–12623.  J. Barbosa, C. Prestipino, O.J. Hernandez, S. Paofai, C. Dejoie, M.G. Viry, C. Boulanger, Inorg. Chem. 58 (2019) 2158–2168.  S. Seghir, C. Boulanger, S. Diliberto, J.M. Lecuire, M. Potel, O.M. Conanec, Electrochem. Commun. 10 (2008) 1505–1508.  M.S. Chae, J.W. Heo, S.C. Lim, S.T. Hong, Inorg. Chem. 55 (2016) 3294–3301.  Y. Cheng, L. Luo, L. Zhong, J. Chen, B. Li, W. Wang, S.X. Mao, C. Wang, V. L. Sprenkle, G. Li, J. Liu, ACS Appl. Mater. Interfaces 8 (2016) 13673–13677.  Z. Jian, Y.S. Hu, X. Ji, W. Chen, Adv. Mater. 29 (2017) 1601925.  C. Masquelier, L. Croguennec, Chem. Rev. 113 (2013) 6552–6591.  P.N. Didwal, R. Verma, C.W. Min, C.J. Park, J. Power Sources 413 (2019) 1–10.  X. Liu, E. Wang, G. Feng, Z. Wu, W. Xiang, X. Guo, J. Li, B. Zhong, Z. Zheng, Electrochim. Acta 286 (2018) 231–241.  G. Li, Z. Yang, Y. Jiang, C. Jin, W. Huang, X. Ding, Y. Huang, Nano Energy 25 (2016) 211–217.  W. Song, X. Ji, Z. Wu, Y. Yang, Z. Zhou, F. Li, Q. Chen, C.E. Banks, J. Power Sources 256 (2014) 258–263.  W. Song, Z. Wu, J. Chen, Q. Lan, Y. Zhu, Y. Yang, C. Pan, H. Hou, M. Jing, X. Ji, Electrochim. Acta 146 (2014) 142–150.  J. Feng, X. Sun, C. Wu, L. Peng, C. Lin, S. Hu, J. Yang, Y. Xie, J. Am. Chem. Soc. 133 (2011) 17832–17838.